170 Advances in Polymer Science
Editorial Board: A. Abe · A.-C. Albertsson · R. Duncan · K. Dusek · W. H. de Jeu J. F...

Author:
N. Fatkullin | T. Ikehara | H. Jinnai | S. Kawata | R. Kimmich | T. Nishi | Y. Nishikawa | H.-B. Sun

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

170 Advances in Polymer Science

Editorial Board: A. Abe · A.-C. Albertsson · R. Duncan · K. Dusek · W. H. de Jeu J. F. Joanny · H.-H. Kausch · S. Kobayashi · K.-S. Lee · L. Leibler T. E. Long · I. Manners · M. Mller · O. Nuyken · E. M. Terentjev B. Voit · G. Wegner

Advances in Polymer Science Recently Published and Forthcoming Volumes

Advanced Computer Simulation Approaches for Soft Matter Sciences I Volume Editors: Holm, C., Kremer, K. Vol. 173, 2004

Radiation Effects on Polymers for Biological Use Volume Editor: Kausch, H. Vol. 162, 2003

Microlithography · Molecular Imprinting Vol. 172, 2004

Polymers for Photonics Applications II Nonlinear Optical, Photorefractive and Two-Photon Absorption Polymers Volume Editor: Lee, K.-S. Vol. 161, 2003

Polymer Synthesis Vol. 171, 2004 NMR · Coordination Polymerization · Photopolymerization Vol. 170, 2004 Long-Term Properties of Polyolefins Volume Editor: Albertsson, A.-C. Vol. 169, 2004 Polymers and Light Volume Editor: Lippert, T. K. Vol. 168, 2004 New Synthetic Methods Vol. 167, 2004 Polyelectrolytes with Defined Molecular Architecture II Volume Editor: Schmidt, M. Vol. 166, 2004 Polyelectrolytes with Defined Molecular Architecture I Volume Editor: Schmidt, M. Vol. 165, 2004 Filler-Reinforced Elastomers · Scanning Force Microscopy Vol. 164, 2003 Liquid Chromatography · FTIR Microspectroscopy · Microwave Assisted Synthesis Vol. 163, 2003

Filled Elastomers · Drug Delivery Systems Vol. 160, 2002 Statistical, Gradient, Block and Graft Copolymers by Controlled/ Living Radical Polymerizations Authors: Davis, K.A., Matyjaszewski, K. Vol. 159, 2002 Polymers for Photonics Applications I Nonlinear Optical and Electroluminescence Polymers Volume Editor: Lee, K.-S. Vol. 158, 2002 Degradable Aliphatic Polyesters Volume Editor: Albertsson, A.-C. Vol. 157, 2001 Molecular Simulation · Fracture · Gel Theory Vol. 156, 2001 New Polymerization Techniques and Synthetic Methodologies Vol. 155, 2001 Polymer Physics and Engineering Vol. 154, 2001

NMR · 3D Analysis · Photopolymerization

With contributions by N. Fatkullin · T. Ikehara · H. Jinnai · S. Kawata · R. Kimmich T. Nishi · Y. Nishikawa · H.-B. Sun

The series presents critical reviews of the present and future trends in polymer and biopolymer science including chemistry, physical chemistry, physics and material science. It is addressed to all scientists at universities and in industry who wish to keep abreast of advances in the topics covered. As a rule, contributions are specially commissioned. The editors and publishers will, however, always be pleased to receive suggestions and supplementary information. Papers are accepted for “Advances in Polymer Science” in English. In references Advances in Polymer Science is abbreviated Adv Polym Sci and is cited as a journal. The electronic content of APS may be found at http://www.springerLink.com

ISSN 0065-3195 ISBN 3-540-20510-1 DOI 10.1007/b12766 Springer-Verlag Berlin Heidelberg New York

Library of Congress Control Number 2004105251 This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, re-printing, re-use of illustrations, recitation, broadcasting, reproduction on microfilms or in other ways, and storage in data banks. Duplication of this publication or parts thereof is only permitted under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer-Verlag. Violations are liable for prosecution under the German Copyright Law. Springer-Verlag is a part of Springer Science+Business Media springeronline.com Springer-Verlag Berlin Heidelberg 2004 Printed in Germany The use of registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting: Strtz AG, Wrzburg Cover: Knkellopka GmbH, Heidelberg; design&production GmbH, Heidelberg Printed on acid-free paper 02/3020/kk – 5 4 3 2 1 0

Editorial Board

Prof. Akihiro Abe

Prof. S. Kobayashi

Department of Industrial Chemistry Tokyo Institute of Polytechnics 1583 Iiyama, Atsugi-shi 243-02, Japan E-mail: [email protected]

Department of Materials Chemistry Graduate School of Engineering Kyoto University Kyoto 615-8510, Japan E-mail: [email protected]

Prof. A.-C. Albertsson Department of Polymer Technology The Royal Institute of Technology S-10044 Stockholm, Sweden E-mail: [email protected]

Prof. Ruth Duncan Welsh School of Pharmacy Cardiff University Redwood Building King Edward VII Avenue Cardiff CF 10 3XF United Kingdom E-mail: [email protected]

Prof. Karel Dusek Institute of Macromolecular Chemistry, Czech Academy of Sciences of the Czech Republic Heyrovsky´ Sq. 2 16206 Prague 6, Czech Republic E-mail: [email protected]

Prof. Dr. W. H. de Jeu FOM-Institute AMOLF Kruislaan 407 1098 SJ Amsterdam, The Netherlands E-mail: [email protected]

Prof. Prof. Kwang-Sup Lee Department of Polymer Science & Engineering Hannam University 133 Ojung-Dong Taejon 300-791, Korea E-mail: [email protected]

Prof. L. Leibler Matire Molle et Chimie Ecole Suprieure de Physique et Chimie Industrielles (ESPCI) 10 rue Vauquelin 75231 Paris Cedex 05, France E-mail: [email protected]

Prof. Timothy E. Long Department of Chemistry and Research Institute Virginia Tech 2110 Hahn Hall (0344) Blacksburg, VA 24061, USA E-mail: [email protected]

Prof. Ian Manners Department of Chemistry University of Toronto 80 St. George St. M5S 3H6 Ontario, Canada E-mail: [email protected]

Prof. Jean-Franois Joanny Institute Charles Sadron 6, rue Boussingault F-67083 Strasbourg Cedex, France E-mail: [email protected]

Prof. Hans-Henning Kausch c/o IGC I, Lab. of Polyelectrolytes and Biomacromolecules EPFL-Ecublens CH-1015 Lausanne, Switzerland E-mail: [email protected]

Prof. Dr. Martin Mller Deutsches Wollforschungsinstitut an der RWTH Aachen e.V. Veltmanplatz 8 52062 Aachen, Germany E-mail: [email protected]

Prof. Oskar Nuyken Lehrstuhl fr Makromolekulare Stoffe TU Mnchen Lichtenbergstr. 4 85747 Garching, Germany E-mail: [email protected]

VI

Editorial Bord

Dr. E. M. Terentjev

Prof. Gerhard Wegner

Cavendish Laboratory Madingley Road Cambridge CB 3 OHE United Kingdom E-mail: [email protected]

Max-Planck-Institut fr Polymerforschung Ackermannweg 10 Postfach 3148 55128 Mainz, Germany E-mail: [email protected]

Prof. Brigitte Voit Institut fr Polymerforschung Dresden Hohe Straße 6 01069 Dresden, Germany E-mail: [email protected]

Advances in Polymer Science Also Available Electronically

For all customers who have a standing order to Advances in Polymer Science, we offer the electronic version via SpringerLink free of charge. Please contact your librarian who can receive a password for free access to the full articles by registering at: http://www.springerlink.com If you do not have a subscription, you can still view the tables of contents of the volumes and the abstract of each article by going to the SpringerLink Homepage, clicking on “Browse by Online Libraries”, then “Chemical Sciences”, and finally choose Advances in Polymer Science. You will find information about the – Editorial Board – Aims and Scope – Instructions for Authors – Sample Contribution at http://www.springeronline.com using the search function.

Contents

Polymer Chain Dynamics and NMR R. Kimmich · N. Fatkullin . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

1

Emerging Technologies for the 3D Analysis of Polymer Structures H. Jinnai · Y. Nishikawa · T. Ikehara · T. Nishi . . . . . . . . . . . . . . . . . . . . . . 115 Two-Photon Photopolymerization and 3D Lithographic Microfabrication H.-B. Sun · S. Kawata . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 169 Author Index Volumes 101–170 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 275 Subject Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 291

APS (2004) Single Contribution:1--113 DOI 10.1007/b12766 Springer-Verlag 2004

Polymer Chain Dynamics and NMR Rainer Kimmich1 (*) · Nail Fatkullin2 1

Sektion Kernresonanzspektroskopie, Universitt Ulm, 89069 Ulm, Germany [email protected] 2 Department of Molecular Physics, Kazan State University, 420008 Kazan, Tatarstan, Russia

1

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

2 NMR Methods . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 NMR Diffusometry. . . . . . . . . . . . . . . . . . . . . . . 2.1.1 Hahn Spin Echo in the Short Gradient Pulse Limit (dD) . 2.1.1.1 Gaussian Propagators . . . . . . . . . . . . . . . . . . . . . 2.1.1.2 Non-Gaussian Propagators . . . . . . . . . . . . . . . . . . 2.1.2 Hahn Spin Echo for Long Gradient Pulses . . . . . . . . . . 2.1.3 Stimulated Echo . . . . . . . . . . . . . . . . . . . . . . . . 2.1.4 Spin Echoes and Steady B0 Gradients. . . . . . . . . . . . . 2.2 NMR Spin–Lattice Relaxometry. . . . . . . . . . . . . . . . 2.2.1 General Theoretical Background . . . . . . . . . . . . . . . 2.2.2 The Field-Cycling NMR Relaxometry Technique . . . . . . 2.3 Residual Dipolar Broadening and Transverse Relaxation . . 2.3.1 The Anderson/Weiss Approach . . . . . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

5 6 6 8 9 10 10 11 13 14 17 20 21

3 Modeling of Chain Dynamics and Predictions for NMR Measurands 3.1 The Rouse Model. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1.1 Translational Segment Diffusion of a Rouse Chain . . . . . . . . . . . 3.1.2 Spin–Lattice Relaxation of a Rouse Chain . . . . . . . . . . . . . . . . 3.2 The Tube/Reptation Model . . . . . . . . . . . . . . . . . . . . . . . . 3.2.1 The Doi/Edwards Limits . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.2 Echo Attenuation by Reptation . . . . . . . . . . . . . . . . . . . . . . 3.2.3 General Remarks on the Tube/Reptation Model . . . . . . . . . . . . . 3.3 Memory Function Formalisms . . . . . . . . . . . . . . . . . . . . . . 3.3.1 The Generalized Langevin Equation (GLE) . . . . . . . . . . . . . . . 3.3.2 The GLE for the Tagged Macromolecule . . . . . . . . . . . . . . . . . 3.3.2.1 The Potential of the Mean Force and the Memory Matrix . . . . . . . 3.3.2.2 The Rouse Equation of Motion as a Special Case of the GLE . . . . . . 3.4 Renormalized Rouse Models . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 The First Renormalization. . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 The Second Renormalization . . . . . . . . . . . . . . . . . . . . . . . 3.4.3 General Remarks on Renormalized Rouse Models . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

22 24 27 28 29 30 34 35 37 37 39 42 43 45 47 51 55

Experimental Studies of Bulk Melts, Networks and Concentrated Solutions. The Three Components of Polymer Dynamics as Relevant for NMR Relaxometry . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Component A. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Component B . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Component C . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Different Time-scale Approach for the NMR Correlation Function . . . .

57

4 4.1 4.1.1 4.1.2 4.1.3 4.1.4

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

3

57 58 60 61 61

2

R. Kimmich · N. Fatkullin

4.1.5 Average Transverse Relaxation . . . . . . . . . . . . . . . . . . . . . 4.1.5.1 Characteristic Temperature . . . . . . . . . . . . . . . . . . . . . . . 4.1.5.2 Characteristic Molecular Weights . . . . . . . . . . . . . . . . . . . . 4.1.5.3 Crossover from the Melt to Dilute Solutions . . . . . . . . . . . . . . 4.2 Chain-end Dynamics (“Whip Model”) . . . . . . . . . . . . . . . . . 4.3 Free-Volume and Void Effects . . . . . . . . . . . . . . . . . . . . . . 4.4 Evidence for Rouse Dynamics (M<Mc). . . . . . . . . . . . . . . . . 4.5 The Three Regimes of Spin–Lattice Relaxation Dispersion in Entangled Polymer Melts, Solutions, and Networks (M<Mc) . . . 4.5.1 High- and Low-Mode-Number Limits (Dispersion Regions I and II) 4.5.2 Intra- and InterSegment Spin Interactions (Dispersion Region III) . 4.5.3 Mesomorphic Phases . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5.4 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5.5 Networks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.6 Translational Segment Diffusion and Spin Diffusion . . . . . . . . . 4.6.1 Center-of-Mass Diffusion . . . . . . . . . . . . . . . . . . . . . . . . 4.6.2 Anomalous Segment Diffusion . . . . . . . . . . . . . . . . . . . . . 4.6.3 Flip-Flop Spin Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . .

. . . .

. . . .

. . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

62 65 68 70 71 75 76

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

79 85 87 92 95 96 97 97 99 100

. . . .

. . . .

. . . .

. . . .

5 5.1 5.2 5.3

Chain Dynamics in Pores (“Artificial Tubes”) . . . . . . . Diffusion in Pores . . . . . . . . . . . . . . . . . . . . . . . Spin–Lattice Relaxation Dispersion in Pores. . . . . . . . . Theoretical Crossover from Rouse to Reptation Dynamics .

. . . .

101 103 104 105

6

Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

107

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

109

Abstract The universal features of polymer dynamics are specifically represented by laws for (anomalous) segment diffusion and chain relaxation modes. Nuclear magnetic resonance (NMR)-based techniques provide direct access to these phenomena. This in particular refers to NMR relaxation and diffusion studies. Methods suitable for this purpose are described in detail. Three basic classes of polymer dynamics models, namely the Rouse model, the tube/reptation model, and the renormalized Rouse models are outlined and discussed with respect to predictions for NMR measurands. A wealth of experimental NMR data are reviewed and compared with predictions of the model theories. It is shown that characteristic features of all three types of models can be verified in great detail provided that the model premisses are suitably mimicked in the experiments. Rouse dynamics is shown to be relevant for polymer melts with molecular weights below the critical value and for solutions of diminished entanglement effect. Features specific for the renormalized Rouse model reveal themselves in the form of high- and low-mode-number limits of the spin–lattice relaxation dispersion. These results are considered to mirror the analytical structure of the Generalized Langevin Equation. Finally, anomalous-diffusion and relaxation laws characteristic for the tube/reptation model can be perfectly reproduced in experiment if the polymer chains are confined in a nanoporous, solid matrix whereas bulk melts are not in accord with these predictions. The dynamics of chains confined in artificial tubes can be treated analytically assuming a harmonic radial potential for the polymer/wall interaction. These results derived for a real tube closely render the characteristic features of the original Doi/Edwards model predicted for a fictitious tube.

Polymer Chain Dynamics and NMR

3

Keywords NMR · Relaxation · Diffusion · Rouse model · Reptation · Renormalized Rouse model Abbreviations BWR CLF CPMG FID GLE NMR ODF PB PDES PDMS PE PEO PGSE PHEMA PIB PIP PMMC PS PTHF PU RF RRM SGSE ThRRM TRRM WLF

Bloch/Wangsness/Redfield theory contour length fluctuation Carr/Purcell/Meiboom/Gill free-induction decay generalized Langevin equation nuclear magnetic resonance order director fluctuations poly(butadiene) poly(diethylsiloxane) poly(dimethylsiloxane) poly(ethylene) poly(ethylene oxide) pulsed gradient spin echo method poly(hydroxyethylmethacrylate) poly(isobutylene) poly(isoprene) polymer mode-mode coupling model poly(styrene) poly(tetrahydrofurane) phenylurazole radio frequency renormalized Rouse model steady gradient spin echo method three times renormalized Rouse model twice renormalized Rouse model Williams/Landel/Ferry

1 Introduction The objective of this review is to outline the basic theories and models of linear polymer chain dynamics [1], and to demonstrate the potential of NMR (nuclear magnetic resonance) techniques for probing the characteristics of molecular motions in such systems. From the methodological point of view we will mainly focus on field-cycling NMR relaxometry and fieldgradient NMR diffusometry, but will also make some reference to transverse relaxation and the residual dipolar interaction occurring in entangled polymer systems. This combination of methods turned out to be most powerful for the examination of chain modes and the translational diffusion properties of polymer segments and the coil center-of-mass. The techniques referred to are best suited to shed light on almost every aspect of polymer dynamics.

4

R. Kimmich · N. Fatkullin

Particular emphasis will be laid on the experimental verification of features of standard theories of polymer dynamics such as the Rouse model, the tube/reptation model [1] or the renormalized Rouse models. Based on the special conditions under which predictions of these theories match experimental findings well, the application limits and the deficiencies of these models for more general scenarios become obvious and help to ameliorate the underlying model ansatz for chain dynamics. In order to elucidate the universal character of polymer chain dynamics, we will attempt to consider as many different polymer species as possible for which NMR relaxometry and diffusometry data are available. On the other hand this means that we must restrict ourselves predominantly to melts of linear homopolymers with a narrow molecular weight distribution to keep the range of literature referred to at manageable levels. Only where enlightening information is expected will we refer to solutions, networks, and mesomorphic systems in addition to isotropic melts. Empirically the conclusions suggested by the huge amount of experimental NMR data available in the literature provide a complete picture rendering dynamical features in great detail. This is in contrast to the stage of development of model theories where the “many-entangled-excluded-volume-chain” problem still has to be overcome, although promising approaches exist. In particular it will turn out that the theoretical concepts available for this sort of system are unable to describe many experimental details quantitatively. On the other hand, predictions of all model theories referred to in this context will be shown to be compatible with certain experimental findings provided that the sample and measuring conditions are adapted to the scenarios that were anticipated in the theoretical derivations. Apart from the introductory section, the article is subdivided into four major sections: NMR Methods; Modeling of Chain Dynamics and Predictions for NMR Measurands; Experimental Studies of Bulk Melts, Networks, and Concentrated Solutions; and Chain Dynamics in Pores. First, the NMR techniques of interest in this context will be described. Second, the three fundamental polymer dynamics theories, namely the Rouse model, the tube/reptation model, and the renormalized Rouse theories are considered. The immense experimental NMR data available in the literature will be classified and described in the next section, where reference will be made to the model theories wherever possible. Finally, recent experiments, analytical treatments, and Monte Carlo simulations of polymer chains confined in pores mimicking the basic premiss of the tube/reptation model are discussed.

Polymer Chain Dynamics and NMR

5

2 NMR Methods NMR provides a rich variety of methods for polymer studies. This in particular refers to the chemical structure of such compounds. Here we deliberately restrict ourselves to investigations on length scales, where chemical bonds and interactions merely matter indirectly via parameters such as segment lengths or friction coefficients. That is, we are dealing with dynamic properties of Kuhn segment chains for times or frequencies beyond those relevant for fluctuations within Kuhn segments. Any chemical shift-based spectroscopy is beyond the scope of this review. Figure 1 shows a schematic representation of the fluctuation time or angular frequency ranges covered by the methods of interest in this context. We will be referring mainly to field-cycling NMR relaxometry combined with conventional high-field methods, to field-gradient NMR diffusometry, and, to a minor degree, to dipolar broadening-based techniques such as the dipolar correlation effect. For an introduction to these methods the reader is referred to monographs like Ref. [2]. Diffusion in polymers can manifest itself in “normal” or “anomalous” form depending on the time or displacement length scale probed in the experiment. The criterion for this distinction is the time dependence of the mean squared displacement 2 k R /t ð1Þ valid in the form of a power law in random unrestricted media. An exponent k=1 indicates normal diffusion as is expected for center-of-mass diffusion, i.e., root mean square displacements much larger than the Flory radius. On the other hand, k> te=tsNe2, where NeNc/2. Intermolecular entanglement forces effectively localize the macromolecule in a space region in the form of a curved tube of diameter d=bNe around the contour line or primitive path of the chain (see Fig. 7). The tube conformation corresponds to that of a freely jointed chain, that is, the tube conformation has a Gaussian end-to-end length distribution. The characteristic time 1 te ts Ne2 ts Nc2 4

ð65Þ

is called the entanglement time, and Ne is the number of Kuhn segments effectively corresponding to an “entanglement”. Segments moving inside the tube are considered to move in a viscous medium as it is anticipated in the Rouse model. In the interior of the tube, entanglement interactions are assumed to be absent. However, as soon as a segment approaches the tube “walls”, entanglement forces become infinitely large so that the polymer is effectively confined by the topological constraints imposed by the tube. The chain-end segments are excepted from this restraint: they are not subject to entanglement forces and can therefore move isotropically. The consequence is that the chain can migrate in a reptile manner (reptation) into a new conformation completely uncorrelated to that of the initial chain coil. 3.2.1 The Doi/Edwards Limits There are four dynamic processes characterized by the four characteristic time constants of the tube/reptation model (see Fig. 7): the segment fluctuation time ts (given in Eq. 53), the entanglement time te (given in Eq. 65), the (longest) Rouse relaxation time tR (given in Eq. 54), and the (tube) disengagement time td (given below in Eq. 71). With these four time constants, four dynamic limits can be defined, which will be termed the Doi/Edwards limits (I)DE to (IV)DE. Table 1 shows the limiting laws for the mean squared

Polymer Chain Dynamics and NMR

31

Fig. 7. Illustration of a polymer chain (the tagged chain) confined in the fictitious tube of diameter d formed by the matrix. The contour line of the tube is called the primitive path having a random-walk conformation with a step length a=d. The four characteristic types of dynamic processes (dotted arrow lines) and their time constants ts, te, tR, and td defined in the frame of the Doi/Edwards tube/reptation model are indicated

segment displacement and the spin–lattice relaxation time commonly expected on this basis. Figure 7 illustrates the chain processes dominating in the four limits. Limit (I)DE (ts >N, the time dependence of the normal mode relaxation functions can be approximated by an exponential decay as t : ð130Þ Cp ðt Þ ¼ Cp ð0Þ exp tp Otherwise Eq. 117 can be solved only numerically. It was found, that the solution of the equation can be approximated by the stretched exponential (Fig. 10) ( ) t bp Cp ðt Þ Cp ð0Þ exp ; ð131Þ ~tp

Fig. 10. Numerically evaluated, normalized autocorrelation function for the RRM for p=5 together with a fitted curve for a stretched exponential, Eq. 131, and an exponential curve. The stretched-exponential parameter is b5=0.66

50

R. Kimmich · N. Fatkullin

Fig. 11. Mode number dependence of the stretching-parameter bp for the RRM (see Eq. 131) for different entanglement parameters y. The number of Kuhn segments was assumed to be N=100 b

p t and bp is a mode-number-dependent stretching parameðbp Þ p ter (see Fig. 11). G(bp) is the gamma function. In the same limit, the mean squared segment displacement obeys ( 2=5 2 t 2 0:23b for t tRR ~ 1 ; yts Rn ðt Þ ¼ ð132Þ 6DRR t for t tRR 1

where ~tp ¼ G

where DRR ¼

0:21 b2 3p2 yts N 3=2

ð133Þ

is the center-of-mass diffusion coefficient in the RRM. The correlation function of the segment tangent vector calculated in the Markovian approximation is in the low-mode-number limit given by 8 D E < b2 yts 2=5 for t tRR 1 ~ bn ðt Þ ~ bn ð0Þ ’ b2 t n t o : ð134Þ RR : N exp RR for t t1 t 1

These results should be asymptotically correct in the limit N!1 and t >> 0.05(6p)4yts. For finite N, the exponents predicted in Eq. 132 may change slightly due to the stretched exponential decay of Cp(t) given in Eq. 131. The limiting laws for the observables of interest in the frame of this review, the mean squared displacement and the (intrasegment) spin–lattice relaxation rate, are summarized in Table 2 (compare [49]).

Polymer Chain Dynamics and NMR

51

Table 2. Theoretical dependences on time (t), angular frequency (w), molecular mass (M), or number of Kuhn segments (N) predicted by the (once) renormalized Rouse model for the mean squared segment displacement and the intrasegment spin–lattice relaxation time. The factors CI, CIRR, CIIRR, and CIIIRR are frequency and molecular mass independent constants Limit

Rouse

(I)RR

(II)RR

ts > < w0 0:730:05 Mw w (region I ‘‘mesophase’’) T1 / : ð182Þ 0 0:250:05 M w (region II ‘‘isotropic phase’’) > > : w0 0:450:05 (region II ‘‘mesophase’’) Mw w

Polymer Chain Dynamics and NMR

93

The slopes in region II for both the isotropic and the mesomorphic phases are in accordance with data for the spin–lattice relaxation time in the rotating frame, T1p. These results for the ordered mesophase are to be compared with the spin–lattice relaxation dispersion expected for nematic liquid crystals where a power law T1 / n0:5 ðODFÞ

ð183Þ

is predicted for order director fluctuations (ODF) at low frequencies [161– 167]. With nematic compounds this law and the collective fluctuations in the ordered state it represents should show up irrespective of whether it is a monomeric or polymeric substance. This is in contrast to the mesophase of PDES. The monomers of this compound do not show any order because they do not contain mesogenic groups. That is, the order observed in the PDES mesophase must have a thermodynamic background different from that of nematic phases. It is concluded that the modified power laws for spin–lattice relaxation dispersion in the mesophase reflect a modified behavior of chain modes rather than collective fluctuations of ensembles of molecules in ordered domains. This conclusion is corroborated by the identical frequency dispersion of the spin–lattice relaxation times T1 and T1p in the laboratory and in the rotating frames, respectively. If the order in the PDES mesophase would be of a nematic nature and the fluctuations causing dispersion region II consequently would be of the ODF type, the frequency dispersion of T1p should vanish while that of T1 is retained [22]. In this context, a study of the dipolar correlation effect in the mesophase of PDES is of particular interest [168]. Using this technique, it was concluded that the sample consists of defect-enriched areas and ordered domains. The two dynamic states are connected with segments of different mobility, and they fluctuate temporally and spatially. The exchange times between the two mobility states range between 0.1 and 1.0 s in the mesomorphic temperature range. The exchange process between the two environments is slow compared with the transverse relaxation rates so that the two signal components can clearly be distinguished. This is in contrast to spin–lattice relaxation where flip-flop spin diffusion as an additional exchange mechanism mediates averaging over all heterogeneities. Spin–lattice relaxation curves therefore decay mono-exponentially in a wide range [155], whereas the transverse magnetization is subject to a superposition of virtually two exponential functions [168]. As concerns the different power law regimes of spin–lattice relaxation given in Eq. 182, it is not yet known to which of the two segment phases they must be attributed or to what degree exchange averaging matters in this respect.

94

R. Kimmich · N. Fatkullin

Fig. 39. Fraction of the more mobile segments in the mesophase of polydiethylsiloxane (PDES) as a function of the reduced temperature. The solid line represents Eq. 184

The dipolar correlation effect is based on stimulated-echo signals [2] and therefore contains elements both of transverse and longitudinal relaxation. Flip-flop spin diffusion as well as material transport may contribute to the exchange mechanism identified this way. An interesting result of the dipolar correlation effect study is the temperature dependence of the fraction of the more mobile segments which was shown to obey the empirical law (see Fig. 39) [168] T Tc Pa ¼ exp 45 ; ð184Þ T where Tc is the (molecular weight dependent) isotropization temperature. Approaching Tc from below increases the fraction of the more mobile segments exponentially as a function of the reduced temperature. Figure 40 shows an attempt to visualize how the areas of different mobility could arise based on “collapsed” coils. The “gain” in chain mobility in the ordered mesophase is attributed to conformations containing many chain folds compensating the dynamic restrictions entailing the almost nematiclike order in this phase (compare the discussion in context with chain-end dynamics and the statistical physics treatment of chain folds in Ref. [124]).

Polymer Chain Dynamics and NMR

95

Fig. 40. Attempt to schematically represent the ordered mesophase of PDES juxtaposed to the isotropic phase. The “collapsed” coil structure assumed in the mesophase entails chain folds that provide additional motional degrees of freedom and is therefore thermodynamically stabilized in a certain temperature range (compare the statistical physics treatment in Ref. [124]). The shaded ellipses indicate somewhat closer packed, more ordered and less mobile areas in contrast to the more mobile, more distorted chain conformations in regions where many folds accumulate

4.5.4 Solutions The features of entangled polymer dynamics fade upon dilution by a lowmolecular solvent. In other words, the critical molecular weight characteristic for the crossover between Rouse-like and entangled dynamics is growing with the degree of dilution (see Eq. 162). NMR relaxation measurements turned out to be particularly suitable for studies of the dilution process. The crossover from the melt to the dilute solution was already demonstrated with the T2/T1 ratio in Fig. 20. It can also be visualized with the aid of spin– lattice relaxation dispersion of PDMS dissolved in CCl4 as a proton-free solvent. Figure 31d shows corresponding data. Compared to the region II dispersion occurring as one of the characteristics of melts of entangled polymers the spin–lattice relaxation dispersion becomes flatter upon dilution. With a PDMS content of 15% in CCl4 the data can be described by the Rouse model as the incarnation of free-chain dynamics (see Fig. 31d). This may appear surprising since the critical molecular weight for this concentration according to Eq. 162 is below the weightaverage molecular weight of the polymer examined, Mw=423,000, so that entangled dynamics should still apply. On the other hand, all polymer dynamics models unspecifically predict some short-time/high-frequency limit where Rouse-like behavior should dominate (see Tables 1–3). In melts of entangled polymers such a regime could never be identified by spin–lattice relaxation dispersion because component B in the form of the high-mode-number limit (region I) appears to overlap with the local segment fluctuation regime (manifesting itself as com-

96

R. Kimmich · N. Fatkullin

ponent A). That is, there is no intermediate time or frequency window left in entangled melts where Rouse dynamics could develop in full. Such a dynamic gap obviously arises in solutions if the polymer concentration is low enough. Component A representing local segment fluctuations becomes accelerated upon dilution, whereas the entanglement effect on the chain modes is shifted to correspondingly longer length and time scales. That is, a very important theoretical requirement is satisfied in this way. We will come back to the topological constraint problem later in the review. 4.5.5 Networks Permanent or thermoreversible cross-links mediate the opposite effect on chain dynamics compared with dilution by a solvent: instead of releasing topological constraints by dilution, additional hindrances to chain modes are established by the network. With respect to NMR measurands relatively large cross-link densities are needed to affect chain modes visible in the experimental time/frequency window, as demonstrated with proton spin–lattice relaxation dispersion of polyethylene cross-linked by 10-Mrad irradiation with electron beams [123] and with styrene–butadiene rubbers [29]. However, there is a very strong effect on the dipolar correlation effect which probes much slower motions and can therefore be used favorably for the determination of the cross-link density [29, 176, 177]. In the plot shown in Fig. 31e, spin–lattice relaxation dispersion curves of permanently cross-linked PDMS are shown. With decreasing mesh length, the chain modes appear to be shifted to lower frequencies. This is indicated by lower values of the relaxation times while the dispersion slopes of regions I and II are retained. On the other hand, the effect on the crossover frequency is minor. The fact that the dispersion regions I, II, and III of proton spin–lattice relaxation retain their qualitative appearance in the presence of (in this case thermoreversible) cross-links is demonstrated in Fig. 34. The influence of fluctuating cross-links on the dispersion curves can be explained by an effectively modified monomeric friction coefficient [131]. A result of particular interest is the shift of the crossover frequencies between dispersion regions I, II, and III. The shifts can be explained by the ratios nI;II nII;III ~ts ¼ ¼ ; ~nI;II ~nII;III ts

ð185Þ

where the quantities with tilde refer to networks. The friction effect on segment fluctuations equally slows down chain modes at the lowest frequencies.

Polymer Chain Dynamics and NMR

97

4.6 Translational Segment Diffusion and Spin Diffusion The NMR diffusometry techniques described in this article are frequently and suitably used for tests of the limits for the mean squared segment displacement predicted by polymer theories. The time and length scales probed by the techniques can be adjusted by the corresponding pulse intervals and the field gradient strength (the “wave number”), respectively. In this way, one gets access to the center-of-mass diffusion limit as well as to the anomalous-segment diffusion regime. The root mean squared displacements examined in the former case are larger than the coil dimension, whereas the latter limit is probed if the displacements are shorter than the coil extension. 4.6.1 Center-of-Mass Diffusion NMR diffusometry is suitable for studies of the center-of-mass diffusion coefficient provided that the diffusion time can be chosen longer than the terminal relaxation time. In terms of the tube/reptation model, this is limit (IV)DE defined by t>>td. Eq. 75 suggests D/Mw2.0 which appears to have been verified several times in experiment [8, 148–150, 169–171]. Figure 41 shows polydimethylsiloxane melt data as a typical example [8]. Data for other polymer melt examples reported in the literature refer to polystyrene and polyethylene at different temperatures [169, 148, 149], and polyethyleneoxide [11, 170]. It appears that all those data perfectly corroborate the validity of limit (IV)DE of the tube/reptation model. However, there are four reasons why the molecular weight dependence observed in experiments may be modified by factors other than the tube constraints: – The condition t>>td is difficult to achieve with high molecular weights so that the anomalous segment displacement regime may gain an increasing influence from low to high molecular weights, as was clearly demonstrated at least with the two highest molecular weights in the plot shown in Fig. 41 [8]. The consequence is an apparently weaker molecular weight dependence. The crossover regime between the center-of-mass and the anomalous segment displacement regimes was extensively studied [172] for polystyrene solutions. It appears that the center-of-mass diffusion coefficient cannot be evaluated reliably by the field-gradient technique without considering the crossover to the anomalous diffusion regime at the same time. – Free volume connected with chain-end blocks influences the molecular weight dependence of chain dynamics in the vicinity of Mc. An apparently steeper molecular weight dependence results on these grounds particularly below Mc. The failure of NMR techniques to directly render the molecular

98

R. Kimmich · N. Fatkullin

Fig. 41. Center-of-mass diffusion coefficient in polydimethylsiloxane (PDMS) melts at 20.5 C [8] as a function of the molecular weight. This self-diffusion coefficient is relevant for root mean square displacements exceeding the random-coil dimension. The experimental condition is that the echo attenuation is recorded with small field-gradient strengths and correspondingly long diffusion times. The straight line represents the law D/Mw2 which seemingly coincides with the prediction by the tube/reptation model for limit (IV)DE (see Eq. 75). The deviation from the Mw2 dependence above Mw=100,000 is due to the fact that in this case the diffusion time could not be chosen long enough to ensure center-of-mass diffusion. Actually we are here already in the anomalous segment diffusion regime. For Mw=250,000, for instance, the root mean square displacement reached along the gradient direction in a diffusion time of 30 ms is only 20 nm compared with a radius of gyration of 25 nm

weight dependence D/Mw1.0 predicted for the Rouse model (see Eq. 59) was explained in this way [148, 149]. – At very high molecular weights, when the diffusion coefficient due to flipflop spin diffusion of the order 1015 m2/s is getting comparable to the ordinary Brownian self-diffusion coefficient, a flatter chain length dependence of the effective diffusion coefficient is expected [10].

Polymer Chain Dynamics and NMR

99

– If very broad, the molecular weight distribution may influence the (average) center-of-mass diffusion coefficient evaluated from echo attenuation curves [169, 175].

In view of the contour-length fluctuation mechanism suggested by Doi as an explanation of the fractional exponent of the power law for the zero-shear viscosity [142], h/Mw3.4, a molecular weight dependence somewhat stronger than predicted by Eq. 75 was predicted also for the center-of-mass diffusion coefficient [169]. More recent studies mainly carried out with concentrated solutions even suggest power laws with universally stronger molecular weight dependences than predicted by the tube/reptation model [172–174]: D / Mw2:40:1 f1:80:2 ; h / Mw3:40:1 f3:80:2 ;

ð186Þ

where f is the volume fraction of the polymer. 4.6.2 Anomalous Segment Diffusion Because of the relatively short displacement time or length scales typically probed by NMR diffusometry, it is particularly well suited to detect anomalies in the segment displacement behavior expected on a time scale shorter than the terminal relaxation time, that is for root mean squared displacements shorter than the random-coil dimension. All models discussed above unanimously predict such anomalies (see Tables 1–3). Therefore, considering exponents of anomalous mean squared displacement laws alone does not provide decisive answers. In order to obtain a consistent and objective picture, it is rather crucial to make sure that (i) the absolute values of the mean squared segment displacement or the time-dependent diffusion coefficient are compatible with the theory, (ii) the dependence on other experimental parameters such as the molecular weight are correctly rendered, and (iii) the values of the limiting time constants are not at variance with those derived from other techniques. For instance, the segmental friction coefficient or the mean squared endto-end distance can be determined directly from viscoelasticity or neutron scattering data. Estimating segment diffusion with the aid of the tube/reptation model based on such data leads to unrealistic predictions. The predicted segment displacements tend to be much too large [9, 12, 178]. Figure 42 shows polyethyleneoxide data as an example. One identifies a time dependence D(t)/t0.5 at short diffusion times in contrast to the law D(t)/t3/4 predicted for te 0.1 s is due to flip-flop spin diffusion which physically limits the detection of molecular displacements by NMR diffusometry

(compare Fig. 44) using the formalism specifically derived for the tube/reptation model (see Eqs. 76–79). In the frame of the experimental accuracy, it is not possible to describe the whole family of echo attenuation curves on the basis of the unmodified predictions in the full diffusion time range for all molecular weights at the same time [9, 12, 178], even if flip-flop spin diffusion (see the following section) is taken into account. On the other hand, if a static “tube” really exists as anticipated in the tube/reptation model, the predictions for anomalous segment diffusion are adequate, of course, and can be verified in experiment. This will be demonstrated by considering linear polymers confined in nanopores. 4.6.3 Flip-Flop Spin Diffusion Flip-flop spin diffusion is a phenomenon specific for NMR. It does not matter with other techniques. Spin diffusion based on Zeeman energy conserving flip-flop transitions of dipolar coupled spins, that is interchange of spin-

Polymer Chain Dynamics and NMR

101

up and spin-down states, is normally negligible compared to molecular selfdiffusion in liquids. However, with viscous systems with little motional averaging of dipolar coupling and with the aid of very strong field gradients, NMR diffusometry is able to detect this immaterial transport mechanism competing with molecular diffusion. Spin echoes can be attenuated on this basis just as with any other incoherent displacement process [181]. Employing the strong fringe-field gradient of a superconducting magnet, it was possible to demonstrate the influence of flip-flop spin diffusion on the echo attenuation of polymer melts [10, 12]. The experiments were carried out by diluting the polymer under investigation isotopically. That is, undeuterated polymers were dissolved in a perdeuterated matrix of polymers of equivalent molecular weight. The reduction of intermolecular dipolar interactions diminishes the proton spin flip-flop rate as expected. The effect is also evident in Fig. 42 referring to a polyethyleneoxide melt with an extremely large molecular weight, Mw=5,000,000. The time-dependent diffusion coefficient was evaluated in the low wave number approximation, Eq. 27, according to hR2(t)i=6D(t)t. The time-independent plateau appearing at times t >> 0.1 s was shown to be due to flip-flop spin diffusion [10, 12]. As a consequence, the proper evaluation of segment diffusion at long diffusion times turned out to be more complicated than often anticipated. However, even with flip-flop spin diffusion theoretically taken into account, it is not possible to fit the formulas predicted by the tube/reptation model to the experimental data with respect to both the time and molecular weight dependences in a consistent way and without assuming unrealistic parameters [12].

5 Chain Dynamics in Pores (“Artificial Tubes”) The motivation to study the dynamics of polymer chains confined in nanoporous materials with more or less rigid pore walls is twofold. Firstly, there may be important technological applications requiring knowledge on the dynamic behavior of polymers under such conditions [182]. The second reason making this field intriguing for polymer science is the possibility to study chain dynamics under topological model constraints in the form of artificial tubes. In the following we will focus on this latter point. The tube introduced in the frame of the Doi/Edwards reptation model for the treatment of bulk systems of entangled polymers is a fictitious one. As outlined above, the laws predicted on this basis (see Table 1) can provide only a rather crude picture failing to account for numerous experimental findings quantitatively as well as qualitatively. It may therefore be helpful to study chain dynamics in tube-like pores of a physically real nature.

102

R. Kimmich · N. Fatkullin

The diffusion and relaxation behavior of diverse oligomers and polymers has been studied in nanoporous silica glasses [183]. Both measuring techniques provide clear evidence for modified chain dynamics compared with the bulk. However, the problem with this sort of system is that interactions of the polymers with the pore walls play an important role and must be distinguished from the geometrical confinement effect. A corresponding analysis was possible by comparison of polymer data with data obtained with short oligomers of the same chemical species. In contrast to the polymers, the oligomers were assumed to be subject to adsorption but not to modifications of the chain modes by geometrical confinement. Subtraction of the oligomer relaxation rates from those measured with polymers in the pores suggests a spin–lattice relaxation dispersion reduced for the influence of geometrical confinements on the chain-mode distribution. Actually a power law dispersion reproducing that predicted for limit (II)DE of the tube/reptation model (see Table 1) could be elucidated this way. A more direct verification of tube/reptation features was possible with systems where the solid matrix and the mobile polymer chains confined to nanopores are of similar organic chemical composition. In the experiments referred to in the following, linear polymers were confined in a solid, that is strongly cross-linked, polymer environment. Under such conditions, the geometry effect can be expected to dominate whereas the wall adsorption phenomenon is of negligible influence. This sort of system was prepared in the form of so-called semiinterpenetrating networks. Preparation details are described in Ref. [184]. The matrix

Fig. 43. Transmission electron micrograph of a replica of a freeze-fractured surface of polyethyleneoxide Mw=6,000 in PHEMA [11]. The pore channels have a width of about 10 nm

Polymer Chain Dynamics and NMR

103

consisted of cross-linked polyhydroxyethyl methacrylate (PHEMA). Linear polyethyleneoxide (PEO) was incorporated in the 10-nm pores. The molecular weights of the PEO samples used in experiment were chosen large enough to ensure that the root mean squared random-coil diameter in bulk exceeds the pore diameter. Figure 43 shows an electron micrograph of pore channels in this material having a width of about 10 nm. 5.1 Diffusion in Pores Segment diffusion in pores suggests itself as a typical model scenario representing the premisses of the tube/reptation model. NMR diffusometry is suitable to probe the time or length scales of the Doi/Edwards limits (II)DE, (III)DE and beyond. Since the wall adsorption effect in the PHEMA system is expected to be negligible, one can therefore expect that the reptation features of the anomalous segment diffusion regime, especially with respect to limit (III)DE, are faithfully rendered by the experiments. Figure 44 shows typical echo attenuation curves recorded with PEO in a solid PHEMA matrix [186]. The good coincidence of the theoretical curves calculated on the basis of Eqs. 76–79 for all accessible values of the experimental parameters k and t for different molecular weights [11] corroborates the validity of the tube/reptation model for linear polymers confined to arti-

Fig. 44. Echo attenuation curves for polyethyleneoxide, Mw=11,200, confined to PHEMA pores at 80 C as a function of the squared wave number, k2, for different diffusion times. The solid lines represent a fit of Eqs. 76–79 to the experimental data. The tube diameter is found to be a=(9€1) nm as the only fitting parameter. Other parameter values such as N=Mw/853, D0=9.661010 m2/s, and b=8.381010 m were taken from the literature [180, 187]

104

R. Kimmich · N. Fatkullin

ficial nanopores in a solid matrix. Very remarkably the tube diameter a (as the only free parameter) fitted to the diffusion data coincides with the pore diameter determined with other techniques such as electron microscopy, Xray scattering or NMR spin diffusion [184]. 5.2 Spin–Lattice Relaxation Dispersion in Pores Field-gradient NMR diffusometry experiments tend to be largely dominated by the time and length scales of limit (III)DE. On the other hand, the much shorter time scale of limit (II)DE can specifically be examined by NMR relaxometry, which under suitable conditions can indirectly probe translational diffusion of polymer segments. The laws predicted in Table 1 for anomalous segment diffusion on the one hand and spin–lattice relaxation on the other are based on the very same translational segment displacement mechanisms. They stipulate each other compellingly. Spin–lattice relaxation at low frequencies, as they can be covered with the aid of field-cycling NMR relaxometry, is therefore suitable to extend the range of field-gradient NMR diffusometry toward much shorter times. The total proton frequency range that can be probed by NMR spin–lattice relaxation techniques is 103 Hz < n < 109 Hz. For the present application, deuteron resonance selectively applied to perdeuterated polymers confined to the pores is superior to proton resonance which, unlike the situation in field-gradient experiments, is affected by signals from the matrix and flipflop spin diffusion across the matrix. The deuteron frequency range is shifted by a factor of 0.15 to lower frequencies. This frequency window largely matches the time scale of chain modes of polymers with medium molecular masses. The exceptional frequency and molecular weight dependence for the spin–lattice relaxation time expected for limit (II)DE, T1 / M0 w3=4 ðwts 1 wte Þ

ð187Þ

(see Table 1), is particularly indicative for reptational segment diffusion. Figure 45a shows the frequency dependence of the deuteron spin–lattice relaxation time of perdeuterated PEO of different molecular weights in a solid PHEMA matrix [95,185]. In the frequency regime, where the standard Bloch/Wangsness/Redfield relaxation theory is applicable, the law given in Eq. 187 is reproduced as T1 / Mw00:05 n0:750:02 :

ð188Þ

The experimental deuteron frequency range in which this frequency dependence was observed is 5105 Hz < n < 6107 Hz. De Gennes prediction for limit (II)DE has thus been verified for polymers confined in artificial

Polymer Chain Dynamics and NMR

105

Fig. 45a, b. Frequency dependence of the deuteron spin–lattice relaxation time of perdeuterated PEO confined in 10-nm pores of solid PHEMA at 80 C (a) and in bulk melts (b) [95, 185]. The dispersion of the confined polymers verifies the law T1 / Mw0 w0:75 at high frequencies as predicted for limit (II)DE of the tube/reptation model (see Table 1). The low-frequency plateau observed with the confined polymers indicates that the correlation function implies components decaying more slowly than the magnetization relaxation curves, so that the Bloch/Wangsness/Redfield relaxation theory [2] is no longer valid in this regime. The plateau value corresponds to the transverse relaxation time, T2, for deuterons extrapolated from the high-field value measured at 9.4 T

tubes in full accordance with the theory. This is in contrast to the bulk behavior of the very same polymers studied with deuteron resonance again. The data in Fig. 45b reproduce features observed with proton and deuteron resonance with bulk melts of other polymer species as discussed above (see Figs. 35 and 36). Polymer chains in bulk melts must obviously have additional degrees of freedom not existing under pore confinements. 5.3 Theoretical Crossover from Rouse to Reptation Dynamics The theoretical background of the confinement effect in (artificial) tubes was recently examined in detail with the aid of an analytical theory as well as with Monte Carlo simulations [70]. The analytical treatment referred to a polymer chain confined to a harmonic radial tube potential. The computer simulation mimicked the dynamics of a modified Stockmayer chain in a tube with “hard” pore walls. In both treatments, the characteristic laws of the tube/reptation model were reproduced. Moreover, the crossover from reptation (tube diameter equal to a few Kuhn segment lengths) to Rouse dy-

106

R. Kimmich · N. Fatkullin

Fig. 46. Theoretical mean squared segment displacement of a chain confined in a randomly coiled tube versus time according to the harmonic radial potential theory [70]. The tube diameter d is given in multiples of the Kuhn segment length b. The crossover tendency to free, unconfined Rouse chain dynamics with increasing tube diameter is obvious. The mean squared displacement is given in units b2, the diffusion time t in units of the segmental fluctuation time ts. The chain length was assumed to be N=1,600 Kuhn segments. The three “anomalous” Doi/Edwards limits (see Table 1) are reproduced with finite tube diameters

namics (tube diameter “infinite”) was demonstrated by varying the tube diameter. Figure 46 shows the time dependence of the mean squared segment displacement as predicted by the harmonic radial potential theory [70]. The three anomalous diffusion limits, (I)DE, (II)DE, and (III)DE, of the tube/reptation model are well reproduced. Note the extended width of the transition regimes between these limits, which should be kept in mind when discussing experimental data with respect to a crossover between different dynamic limits. Increasing the effective tube diameter is accompanied by the gradual transition to Rouse-like dynamics of an unconfined chain (where entanglement effects are not considered). The spin–lattice relaxation dispersion was derived with the same sort of theory. Figure 47 shows data obtained under the same conditions as assumed for the mean squared displacement data in Fig. 46. Again the dispersion most specific for the tube/reptation model, namely T1/w0.75 which is predicted for limit (II)DE, was perfectly reproduced at low frequencies.

Polymer Chain Dynamics and NMR

107

Fig. 47. Spin–lattice relaxation dispersion for a chain of N=1,600 Kuhn segments (of length b) confined to a randomly coiled tube with a harmonic radial potential with varying effective diameters d˙. The data were calculated with the aid of the harmonic radial potential theory [70]. ~c is a constant. At low frequencies the curves visualize the crossover from Rouse dynamics depending on the effective tube diameter. The latter case is described by a T1 dispersion proportional to w3/4 characteristic for limit (II)DE of the tube/ reptation model

6 Concluding Remarks NMR may be considered as a particularly versatile class of investigation methods suitable for polymer dynamics studies. In particular, field-cycling NMR relaxometry employed in parallel with field-gradient NMR diffusometry is an unmatched combination of methods for the elucidation of features of chain dynamics. A great wealth of clearly documented phenomena for different measurands, experimental parameters, and different polymer species in different environments and under different thermodynamic conditions were discovered, and appear to be suitable for direct comparisons with theoretical model predictions. One can say that the experimental data available so far already render a closed picture from the empirical point of view. Transverse and longitudinal NMR relaxometry of 1H and 13C nuclei was shown to be governed by three components of chain dynamics. With respect to tests of theoretical model concepts, the most important one is component B which reflects the influence of chain modes and can be probed with the field-cycling technique. Field-gradient NMR diffusometry is suitable for recording translational displacement properties by self-diffusion. This in particular refers to the anomalous segment displacement regime. Center-of-mass diffusion is also accessible this way but must be handled with some care because of the experimental limitation of the maximum diffusion time. Furthermore the in-

108

R. Kimmich · N. Fatkullin

fluence of flip-flop spin diffusion must be taken into account when examining long polymers. Three basic model theories have been considered: the Rouse model, the tube/reptation concept, and the renormalized Rouse formalism. Depending on the sample system and the experimental conduct, characteristic features of all these theories have been shown. Some spectacular predictions of theories were verified, others were ruled out. The frequency dependence of the spin–lattice relaxation time predicted by the Rouse model was verified with polymer melts for Mw<Mc in accordance with the segmental fluctuation time determined from the T1 minimum condition. Melts with Mw>>Mc did not show any such behavior in the shorttime limit although predicted so by all three model theories. On the other hand, dilution of the polymer by a low-molecular solvent increases Mc and diminishes the entanglement effect. Under such conditions, Rouse-like behavior was observed. The tube/reptation model of entangled polymer dynamics suggests a number of peculiar anomalous-diffusion limits that were consistently and quantitatively verified in artificial tubes of a solid porous matrix with the aid of field-cycling NMR relaxometry and field-gradient NMR diffusometry. This clear corroboration of a model prediction is however in contrast to the dynamics concluded for bulk melts. In that case neither the prediected T1 dispersion nor the anomalous segment diffusion behavior was found with respect to the frequency and molecular weight dependences. The assumption of static fictitious tubes as a replacement scheme for the entangling matrix effect is obviously too crude for bulk melts, and does not render the features of polymer dynamics correctly. Based on the generalized Langevin equation, the renormalized Rouse models suggest dynamic high- and low-mode-number limits as an implicit structural feature of this equation of motion. This is a stand-alone prediction of paramount importance independent of any absolute values of power law exponents that arise and are measured in the formalism and in experiment, respectively. The two limits manifesting themselves as power law spin–lattice relaxation dispersions were clearly identified in bulk melts of entangled polymers of diverse chemical species. Apart from these two relaxation dispersion regimes, which are mainly based on intrasegment spin interactions (and possibly nearest neighbor intersegment contributions), a third dispersion region specific for dipolarcoupled nuclei exists at low frequencies. This was shown to be due to (longdistance) dipolar interactions being relevant for protons but not for deuterons. A most important finding in general and for establishing of model theories is the fact that segment dynamics is affected by microstructural details already at relatively short times. The local fluctuations of a Kuhn segment typically occur on a time scale shorter than 1010 s and on a length scale of

Polymer Chain Dynamics and NMR

109

up to 1 nm. It was shown that factors such as chain entanglements, crosslinking or mesomorphic order quite amazingly, and contrary to most model expectations, have an influence on segment dynamics already rather close to these time and length scales. This finding became evident from the relaxometry studies reported and was also observed in the literature [129]. On the other hand, chain modes with low mode numbers and even global, molecular weight dependent motions corresponding to chain relaxation times beyond the Rouse relaxation time do show up at the predicted time and length scales. Acknowledgments We thank Elmar Fischer, Alexei Denissov, Margarita Kroutieva, Hans Wiringer, and Birgit K rner for discussions and excellent assistance in the preparation phase of this article. Grants by the DFG, the Volkswagen-Stiftung, CRDF, and RFBR are gratefully acknowledged.

References 1. Doi M, Edwards SF (1986) The theory of polymer dynamics. Clarendon, Oxford 2. Kimmich R (1997) NMR tomography, diffusometry, relaxometry. Springer, Berlin Heidelberg New York 3. Fatkullin N, Kimmich R (1995) Phys Rev E 52:3273 4. Torrey HC (1956) Phys Rev 104:563 5. Stejskal EO, Tanner JE (1965) J Chem Phys 42:288 6. Tanner JE, Stejskal EO (1968) J Chem Phys 49:1768 7. Saarinen TR, Johnson CS (1988) J Magn Reson 78:257 8. Kimmich R, Unrath W, Schnur G, Rommel E (1991) J Magn Reson 91:136 9. Fischer E, Kimmich R, Fatkullin N (1996) J Chem Phys 104:9174 10. Fischer E, Kimmich R, Fatkullin N (1997) J Chem Phys 106:9883 11. Fischer E, Kimmich R, Beginn U, M ller M, Fatkullin N (1999) Phys Rev E 59:4079 12. Fischer E, Kimmich R, Fatkullin N, Yatsenko G (2000) Phys Rev E 62:775 13. Fujara F, Geil B, Sillescu H, Fleischer G (1992) Z Phys B 88:195 14. Kimmich R, Fischer E (1994) J Magn Reson A 106:229 15. Kimmich R, Fischer E, Callaghan P, Fatkullin N (1995) J Magn Reson A 117:53 16. Grinberg F, Kimmich R (1995) J Chem Phys 103:365 17. Abragam A (1961) The principles of nuclear magnetism. Clarendon, Oxford 18. Kimmich R (1980) Bull Magn Reson 1:195 19. Noack F (1986) Progr NMR Spectr 18:171 20. Kimmich R (1996) Molecular motions: T1 frequency dispersion in biological systems. In: Grant DM, Harris RK (eds) Encyclopedia of nuclear magnetic resonance, vol 5. Wiley, Chichester, pp 3083–3088 21. Seitter R, Kimmich R (1999) Magnetic resonance: relaxometers. In: Lindon J, Trantar G, Holmes J (eds) Encyclopedia of spectroscopy and spectrometry. Academic, London, pp 2000–2008 22. Anoardo E, Grinberg F, Vilfan M, Kimmich R (2004) Chem Phys 297:99 23. Cohen-Addad JP (1993) Progr NMR Spectr 25:1 24. Guillermo A, Cohen-Addad JP, Bytchenkoff D (2000) Chem Phys 113:5098 25. Cohen-Addad JP, Guillermo A (2000) Phys Rev Lett 85:3432

110

R. Kimmich · N. Fatkullin

26. Brereton MG (1990) Macromolecules 23:1119 27. Ball RC, Callaghan PT, Samulski ET (1997) J Chem Phys 106:7352 28. Callaghan PT, Samulski ET (1998) Macromolecules 31:3693 29. Fischer E, Grinberg F, Kimmich R, Hafner S (1998) J Chem Phys 109:846 30. Maxwell RS, Balazs B (2002) J Chem Phys 116:10492 31. Graf R, Heuer A, Spiess HW (1998) Phys Rev Lett 80:5738 32. Dollase T, Graf R, Heuer A, Spiess HW (2001) Macromolecules 34:298 33. Schnur G, Kimmich R (1988) Chem Phys Lett 144:333 34. K pf M, Schnur G, Kimmich R (1988) J Polym Sci Polym Lett 26:319 35. Kimmich R, Schnur G, K pf M (1988) Progr NMR Spectr 20:385 36. Kimmich R, K pf M, Callaghan P (1991) J Polym Sci Polym Phys 29:1025 37. Volkenstein MV (1963) Configurational statistics of polymer chains. Interscience, New York 38. Birshtein TM, Pticin OB (1966) Conformation of macromolecules. Interscience, New York 39. Flory PG (1969) Statistical mechanics of chain molecules. Interscience, New York 40. Yamakava H (1971) Modern theory of polymer solutions. Harper and Row, New York 41. de Gennes PG (1979) Scaling concepts in polymer physics. Cornell University Press, Ithaka 42. Grosberg AYu, Khokhlov AR (1994) Statistical physics of macromolecules. AIP, New York 43. Gotlib YuYa, Darinskii AA, Svetlov YuE (1986) Physical kinetics of macromolecules. Khimia, Leningrad (in Russian) 44. Grosberg AYu, Khokhlov AR (1997) Giant molecules: here, there, and everywhere... Academic, San Diego 45. Kargin VA and Slonimskii GL (1949) Journal Fizhimii (USSR) 23:563 46. Rouse PJ (1953) J Chem Phys 21:1272 47. Fatkullin N, Kimmich R, Weber HW (1993) Phys Rev E 47:4600 48. Kimmich R, Fatkullin N, Weber HW, Stapf S (1994) J Non-Cryst Solids 172–174: 689 49. Fatkullin N, Kimmich R (1994) J Chem Phys 101:822 50. Khazanovich TN (1963) Polymer Sci USSR 4:727 51. Ullman R (1965) J Chem Phys 43:3161 52. Ferry JD (1980) Viscoelastic properties of polymers. Wiley, New York 53. Edwards SF (1967) Proc Phys Soc 92:9 54. de Gennes PG (1971) J Chem Phys 55: 572 55. Doi M, Edwards SF (1978) J Chem Soc Faraday Trans II 74:1789 56. Klein J (1978) Macromolecules 11:852 57. Doi MJ (1983) Poly Sci Poly Phys 21:667 58. Guenza M (2002) Phys Rev Lett 88:025901 59. Rubinstein M (1987) Phys Rev Lett 59:1946 60. de Cloizeaux (1988) J Europhys Lett 5:437 61. Graessley WW (1982) Adv Polym Sci 47:1 62. Pearson D (1987) Rubber Chem Tech 60:437 63. Marruci G (1985) J Polym Sci Polym Phys 23:159 64. Watanabe H, Tirrel M (1989) Macromolecules 22:927 65. Doi M, Pearson D, Kornfield J, Fuller G (1989) Macromolecules 22:1488 66. Fixman M (1991) J Chem Phys 95:1410 67. Gao J, Weiner JH (1992) Macromolecules 25:1348 68. Gao J, Weiner JH (1994) Science 266:748 69. Loriot G, Weiner JH (1998) J Polym Sci Polym Phys 36:143

Polymer Chain Dynamics and NMR

111

70. Denissov A, Kroutieva M, Fatkullin N, Kimmich R (2002) J Chem Phys 116:5217 71. Kimmich R (1975) Polymer 16:851 72. Kimmich R (2002) Chem Phys 284:253 73. Ardelean I, Kimmich R (2003) Ann Rep NMR Spectr 49:43 74. Fatkullin N, Kimmich R (1999) JETP Lett 69:762 75. Fatkullin N, Kimmich R (1999) Macromol Symp 146:103 76. Padding JT, Briels WJ (2001) J Chem Phys 115:2446 77. Fatkullin N (2002) J Non-Cryst Solids 307–310:824 78. Skolnick J, Kolinski A (1990) Adv Chem Phys 78:223 79. Kremer K, Grest GS (1990) J Chem Phys 92:5057 80. Kremer K, Grest GS (1992) J Chem Soc Faraday Trans 88:1707 81. Pakula T (1996) Recent Res Devel Polym Sci 1:101 82. Binder K, Paul W (1997) J Polym Sci Polym Phys 35:1 83. Pakula T (1998) Computational Theor Polym Sci 8:21 84. Shaffer JS (1995) J Chem Phys 103:761 85. Binder K, Paul W (1997) J Polym Sci Polym Phys 35:1 86. Khalatur PG (1996) Computer simulations in polymer systems. In: Kuchanov SI (ed) Mathematical methods in contemporary chemistry. Gordon and Breach, New York 87. Padding JT, Briels WJ (2002) J Chem Phys 117:925 88. Paul W (2002) Chem Phys 284:59 89. Hermann MF (1990) J Chem Phys 92:2043 90. Hermann MF, Panajotova B, Lorenz KT (1996) J Chem Phys 105:1153 91. Douglas JF, Hubbard JB (1991) Macromolecules 24:3163 92. Chatterjee AP, Loring RF (1995) J Chem Phys 103:4711 93. Ngai KL, Phillies GDJ (1996) J Chem Phys 105:8385 94. Ngai KL (1999) Macromol Symp 146:117 95. Kimmich R, Seitter R-O, Beginn U, M ller M, Fatkullin N (1999) Chem Phys Letters 307:147 96. Zwanzig R (1974) J Chem Phys 60:2717 97. Bixon M, Zwanzig R (1978) J Chem Phys 68:1890 98. Schweizer KS (1989) J Chem Phys 91:5802 99. Schweizer KS (1989) J Chem Phys 91:5822 100. Schweizer KS (1993) Physica Scripta T49:99 101. Fuchs M, Schweizer KS (1997) J Chem Phys 106:347 102. Guenza M, Schweizer KS (1997) J Chem Phys 106:7391 103. Schweizer KS, Fuchs M, Szamel G et al. (1997) Macromol Theory Simul 6:1037 104. Guenza M (1999) J Chem Phys 110:7574 105. Fatkullin N, Kimmich R, Kroutieva M (2000) JETP 91:150 106. Genz U (1994) Macromolecules 27:3501 107. Genz U, Vilgis TA (1994) J Chem Phys 101:7101 108. Genz U, Vilgis TA (1994) J Chem Phys 101:7111 109. Zwanzig R (1960) J Chem Phys 33:1336 110. Zwanzig R (1961) Phys Rev 124:985 111. Mori H (1965) Progr Theor Phys 33:423 112. Mori H (1965) Progr Theor Phys 34:765 113. Hansen JP, McDonald (1991) Theory of simple liquids, 2nd edn. Academic, London 114. Baluccani U, Zoppi M (1994) Dynamics of the liquid state. Clarendon, Oxford 115. Berne BJ, Pecora R (1976) In: Berne BJ (ed) Dynamical light scattering. Wiley, New York 116. Edwards SF, Grant JW (1973) J Phys A Math Nucl Gen 6:1169

112

R. Kimmich · N. Fatkullin

117. Edwards SF, Grant JW (1973) J Phys A Math Nucl Gen 6:1189 118. Ronca G (1983) J Chem Phys 79:1031 119. Fixman MF (1988) J Chem Phys 89:3892 120. Hess W (1988) Macromolecules 21:2620 121. Rostiashvili VG (1990) Sov Phys JETP 70:563 122. Pokrovskii VN (1992) Sov Phys Usp 35:384 123. Kimmich R, Bachus R (1982) Coll Polym Sci 260:911 124. Kimmich R, K pf M (1989) Progr Coll Polym Sci 80:8 125. Weber HW, Kimmich R (1993) Macromolecules 26:2597 126. Gotlib YY, Torchinskii IA, Shevelev VA (2001) Polym Sci A 43:1066 127. Gotlib YY, Torchinskii IA, Shevelev VA (2002) Polym Sci A 44:206 128. Voigt G, Kimmich R (1980) Polymer 21:1001 129. Qui XH, Ediger MD (2002) Macromolecules 35:1691 130. Allen G, Connor TM, Pursey H (1963) Trans Faraday Soc 59:1525 131. Kimmich R, Gille K, Fatkullin N, Seitter R, Hafner S, M ller M (1997) J Chem Phys 107:5973 132. Koch H, Bachus R, Kimmich R (1980) Polymer 21:1009 133. Schneider H, Hiller W (1990) J Polym Sci Polym Phys 28:1001 134. Singer A, Hiller W (1985) Polym Bull 14:469 135. Manelis GB, Erofeev LN, Provotorov BN, Khitrin AK (1989) Sov Sci Rev B Chem 14:1 136. Kuhn W, Barth P, Hafner S, Simon G, Schneider H (1994) Macromolecules 27:5773 137. Cohen-Addad JP, Guillermo A (1984) J Polym Sci Polym Phys 22:931 138. Kimmich R (1984) Polymer 25:187 139. Kimmich R, Rosskopf E, Schnur G, Spohn KH (1985) Macromolecules 18:810 140. Weber HW, Kimmich R, K pf M, Ramik T, Oeser R (1992) Progr Coll Polym Sci 90:104 141. K pf M, Schnur G, Kimmich R (1988) Macromolecules 21:3340 142. Doi M (1981) J Polym Sci Polym Lett 19:165 143. K pf M (1991) PhD thesis, Universitt Ulm 144. Kimmich R (1985) Helv Phys Acta 58:102 145. Doolittle AK (1951) J Appl Phys 22:1471 146. Fox TG, Gratch S, Lashaek S (1956) In: Eirich FR (ed) Rheology, vol.1. Academic, New York, p 431 147. Bailey RT, North AM, Pethrick RA (1981) Molecular motion in high polymers. Clarendon, Oxford 148. Fleischer G (1984) Polym Bull 11:75 149. Fleischer G (1987) Coll Polym Sci 265:89 150. von Meerwall E, Ferguson RD (1982) J Polym Sci Polym Phys 20:1037 151. Kimmich R, Peters A, Spohn K-H (1981) J Membrane Sci 9:313 152. Bachus R and Kimmich R (1983) Polym Communications 24:317 153. Kimmich R, Weber HW (1993) J Chem Phys 98:5847 154. Kimmich R, Fatkullin N, Seitter R-O, Gille K (1998) J Chem Phys 108:2173 155. Kimmich R, Stapf S, M ller M, Out R, Seitter R-O (1994) Macromolecules 27:1505 156. Link T, Kimmich R (2000) unpublished 157. Fenchenko KV (1997) Polym Sci B 39:146 158. Herman, MF (2000) J Chem Phys 112:3040 159. Godovsky YK, Papkov VS (1989) Adv Polym Sci 88:129 160. K gler G, Loufakis K, M ller M (1990) Polymer 31:1538 161. Pincus P (1969) Solid State Commun 7:415 162. Blinc R, Hogenboom D, OReilly D, Peterson E (1969) Phys Rev Lett 23:969

Polymer Chain Dynamics and NMR

113

163. Doane JW, Johnson DL (1970) Chem Phys Lett 6:291 164. Ukleja P, Pirs J, Doane JW (1976) Phys Rev A 14:414 165. Dong RY (1983) Isr J Chem 23:370 166. Vilfan M, Kogoj M, Blinc R (1987) J Chem Phys 86:1055 167. Zeuner U, Dippel T, Noack F, M ller K, Mayer C, Heaton N, Kothe G (1992) J Chem Phys 97:3794 168. Grinberg F, Kimmich R, M ller M, Molenberg A (1996) J Chem Phys 105:9657 169. Bachus R, Kimmich R (1983) Polymer 24:964 170. Maklakov AI, Skirda VD, Fatkullin NF (1990) Self diffusion in polymer melts and solutions. In: Cheremisinoff NP (ed) Encyclopedia of fluid mechanics, vol 9: polymer flow engineering. Gulf, Houston 171. Manz B, Callaghan PT (1997) Macromolecules 30:3309 172. Komlosh ME, Callaghan PT (1998) J Chem Phys 102:1648 173. Tao H, Lodge TP, von Meerwall ED (2000) Macromolecules 33:1747 174. Lodge TP (1999) Phys Rev Letters 83:3218 175. Fleischer G (1985) Polymer 26:1677 176. Grinberg F, Garbarczyk M, Kuhn W (1999) J Chem Phys 111:11222 177. Garbarczyk M, Grinberg F, Nestle N, Kuhn W (2001) J Polym Sci Polym Phys 39:2207 178. Rommel E, Kimmich R, Sp lbeck M, Fatkullin NF (1993) Progr Colloid Polym Sci 93:155 179. Kugler J, Fischer EW (1983) Makromol Chemie 184:2325 180. Smith GD, Yoon DY, Jaffe RL, Colby RH, Krishnamoorti R, Fetters LJ (1996) Macromolecules 29:3462 181. Fatkullin NF, Yatsenko GA, Kimmich R, Fischer E (1998) J Exp Theor Phys 87:294 182. de Gennes PG (1999) Advan Polym Sci 138:91 183. Stapf S, Kimmich R (1995) Macromolecules 29:1638 184. Beginn U, Fischer E, Pieper T, Mellinger F, Kimmich R, M ller M (2000) J Polym Sci Polym Chem 38:2041 (note that a misprint occurred in that paper with the length scale specified in the electron micrograph given at Fig. 8) 185. Kimmich R, Fatkullin N, Seitter R-O, Fischer E, Beginn U, M ller M (1999) Macromol Symp 146:109 186. Fischer E, Beginn U, Fatkullin N, Kimmich R (2004) Macromolecules 37:3277 187. Graessley WW, Edwards SF (1981) Polymer 22:1329 Editor: Sam Edwards

Received: February 2003

APS (2004) 170:115--113 DOI 10.1007/b95533 Springer-Verlag 2004

Emerging Technologies for the 3D Analysis of Polymer Structures Hiroshi Jinnai1 · Yukihiro Nishikawa1 · Takayuki Ikehara2 · Toshio Nishi3 (*) 1

Department of Polymer Science and Engineering, Kyoto Institute of Technology, 606-8585 Kyoto, Japan [email protected] 2 Department of Applied Chemistry, Faculty of Engineering, Kanagawa University, 3-27-1 Rokkakubashi, Kanagawa-ku, 221-8686 Yokohama, Japan 3 Department of Organic and Polymeric Materials, School of Science and Engineering, Tokyo Institute of Technology, 2-12-1 Ohokayama, Meguro-ku, 152-8551 Tokyo, Japan

1

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

118

2 2.1 2.2

3D Microscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Laser Scanning Confocal Microscopy (LSCM) . . . . . . . . . . . . . . . . . . Transmission Electron Microtomography (TEMT) . . . . . . . . . . . . . . .

120 121 123

3 3.1 3.2 3.2.1 3.2.2 3.2.3 3.3

Digital Image Analysis of 3D Structures. 3D Reconstruction . . . . . . . . . . . . . Curvature Distribution Measurements . . Surface Curvatures . . . . . . . . . . . . . Parallel Surface Method (PSM) . . . . . . Sectioning and Fitting Method (SFM) . . Surface Topology . . . . . . . . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

125 125 126 127 128 129 132

. . . . . .

136 136 137 139 139 141

. . .

144 146 147

. . . . . . . . . .

152 152

. . . . .

154

. . . . .

155

. . . . .

157

4

Time Evolution of Bicontinuous Structure in Spinodal Interface of a Binary Polymer Mixture . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Basics of Phase Separation in Binary Polymer Mixutures . . . . . . . . . . 4.2 Direct 3D Visualization of Phase-Separating Bicontinuous Structures. . . . 4.3 3D Structural Analysis of Phase-Separating Bicontinuous Structures . . . . 4.3.1 Scaled Structure Factor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.2 Interfacial Curvature Measurement: Comparison Between LSCM and TRLS 4.3.3 Curvature Distribution Measurements of Phase-Separating Bicontinuous Structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4 Scaling Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5 Effects of Surface Wetting and Confinement on Spinodal Decomposition . 5

Direct Measurement of Interfacial Curvature Distributions in a Bicontinuous Block Copolymer Nanostructure . . . . . . . . . 5.1 Basics of Microphase-Separated Morphologies in Block Copolymers 5.2 Direct 3D Visualization and Curvature Distribution of Bicontinuous Block Copolymer Nanostructure . . . . . . . . . . . 5.3 Geometrical and Topological Analysis of Bicontinuous Block Copolymer Nanostructure . . . . . . . . . . . 5.3.1 Comparison Between Experiment and Theory in Terms of Interfacial Curvature Distribution . . . . . . . . . . . . . . . . . .

116 6

H. Jinnai et al. Geometrical Similarity/Difference Between Polymer Blend and Block Copolymer Structures. . . . . . . . . . . . . . . . . . . . . . . . .

158

Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

163

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

164

7

This review covers recent progress of studies using new methods for analyzing polymer structures, with emphasis on three-dimensional (3D) microscopy, e.g., laser scanning confocal microscopy (LSCM) and transmission electron microtomography (TEMT). These methods have been applied to morphological studies of structures in polymer alloys over the past few years. We review some of the studies dealing with 3D structures of binary polymer blends and block copolymers that are self-assembled during the phase separation processes and/or phase transition. Typical sizes of such self-assembled structures are of the order of micro- and nanometers, respectively. A great deal of new structural information, which has never been obtained from conventional microscopy or various scattering methods, can be evaluated directly from the 3D volume data. The structural information obtained from 3D microscopy offers essential insight into the physics of nonlinear, nonequilibrium phenomena and the statistical mechanics of long-chain molecules. Keywords Polymer alloy · 3D microscopy · 3D digital image analysis · Bicontinuous structures Abbreviations and Symbols Area of i-th triangles (generated by MCA) sharing the j-th POI Atri(i;j) CMC Constant mean curvature CT Computerized tomography d Signed displacement of the parallel surface D Thickness of (blend) specimen Diameter (size) of an object reconstructed in CT DCT DPB Deuterated polybutadiene f Copolymer composition Styrene volume fraction in microphase-separated structure fS of SIS block copolymer E Number of edges of faces subdividing the surface F Number of faces subdividing the surface F(x) Scaled structure factor f(x,y) Intersection of an object H Mean curvature ~ H Scaled mean curvature hHi Area-averaged mean curvature I(q,t) Scattering intensity in TRLS experiment I(x,y,z) Intensity of fluorescence from a particular point in a focal plane (x–y plane) at a depth z K Gaussian curvature ~ K Scaled Gaussian curvature hKi Area-averaged Gaussian curvature L Crystallographic unit cell edge LS Light scattering

Emerging Technologies for the 3D Analysis of Polymer Structures LSCM MCA N NCT Nj NA Ntri n ntri p PB p(r,j) P(H,K) PH(H) ~H H; ~ t P pi PK(K) ~ t ~K K; P POI PSM q qm(t) qc r RI Rm Rm,LS Rm,LSCM Rg S SCFT SD SFM Si SIS S(q) t TDGL TEM TEMT u and v V Vs z c dA(j)

117

Laser scanning confocal microscopy Marching cubes algorithm Number of pixels along the edge of the image Number of projections in CT Coordination number at a junction Numerical aperture of an objective Total number of triangles comprising interface generated by MCA Normal vectors at vertices of the polygon generated by MCA Normal vector of each triangle generated by MCA Positional vector of a surface Polybutadiene Projection at an angle j Joint probability density of surface curvatures Marginal probability densities of the mean curvature Scaled marginal probability densities of the mean curvature Coordinates of the i-th vertices of the triangle generated by MCA Marginal probability density of the Gaussian curvature Scaled marginal probability density of the Gaussian curvature Point of interest at a surface Parallel surface method Wave number Wave number at which I(q,t) shows a maximum Crossover wave number from q6 to q4 with increasing q in I(q,t) of spinodally decomposing polymer mixtures Resolution of reconstructed image in CT Roughness index Area-averaged mean radius in Tomitas scattering theory Mean radius estimated from LS based on Tomitas scattering theory (Eqs. 28 and 29) Mean radius estimated from LSCM based on Tomitas scattering theory (Eq. 29) Radius of gyration of polymers (Total) interfacial area Self-consistent field theory Spinodal decomposition Sectioning and fitting method Area of i-th neighboring triangles generated by MCA Poly(styrene-b-isoprene-b-styrene) triblock copolymer Scattering structure factor Phase-separation time Time-dependent Ginzburg–Landau equation Transmission electron microscopy Transmission electron microtomography Curvilinear coordinates of a surface Number of vertices of faces subdividing the surface Volume of the whole system Depth along the optical axis of LSCM Euler–Poincar characteristic Local area assigned to j-th POI

118 DF DH DK DZ hh(t)2i q ki l lLS Lm(t) sH P (t) f fPB j

H. Jinnai et al. Full width at half maximum (fwhm) of optical sections in LSCM observations Class interval of H Class interval of K Increment along depth direction of LSCM Mean squared refractive index fluctuations Scattering angle in TRLS experiments Principal curvatures (i=1 and 2) Wavelength of laser of LSCM Wavelength of laser in TRLS experiments Length characterizing the global size of SD bicontinuous structures Standard deviation of the mean curvature distribution Surface area per unit volume Volume fraction of one of the phases in polymer mixture Volume fraction of the PB-rich phase in DPB/PB mixture Angle of the projection slice in computerized tomography (CT)

1 Introduction Polymer materials are ubiquitous in our daily life. Such materials often consist of more than one species of polymer and thus become multicomponent systems, such as polymer blends [1,2] and block copolymers [3]. Due to repulsive interaction between the constituent polymers, the multicomponent polymer materials involve “phase separation”. Studies to characterize the phase-separated structures inside the materials have been growing intensively over the past three decades. Academic interest in the complex fluids (to which polymeric systems belong) as well as ceaseless industrial need for developing new materials activated such studies. In academia, for example, pattern formation and self-assembling processes of binary polymer blends are one of the most fascinating research themes in nonlinear, nonequilibrium phenomena. Block copolymers likewise self-organize into (equilibrium) phase-separated nanostructures (termed “microphase-separated structures” in contrast to the “macrophaseseparated structures” in the polymer blend). Since it is required for the block copolymers to place their junctions at the interface and thus the microdomain-forming blocks must uniformly fill space in the most entropically favored manner, the block copolymer morphologies are often highly organized. Studies of the block copolymer morphologies belong to the statistical mechanics of long-chain molecules. In industry, such phase-separated polymer systems have been found important to achieve superior physical properties. Hence, the structure–property relationship in multicomponent polymeric materials is of significant importance, basic studies on which eventually render new designs of polymer materials satisfying the diverse requirements of industry.

Emerging Technologies for the 3D Analysis of Polymer Structures

119

Up to now, morphological studies of the multicomponent polymeric materials have been carried out by various microscopic and scattering methods. Optical microscopes, transmission electron microscopes (TEM), scanning electron microscopes (SEM), and atomic force microscopes (AFM) are commercially available and widely used. The biggest advantage to using such microscopes is that they offer intuitive real-space representation of morphologies by showing images. However, when it comes to “measurements”, especially in a quantitative way, the microscopes sometimes give only limited pieces of structural information with inferior statistical accuracy compared with scattering methods. The scattering techniques give statistically averaged structural information over the scattering volume, which is normally a lot bigger than the area of the microscopes. Although accurate, the scattering methods do not directly provide intuitive insight into the morphologies. Moreover, in general, the scattering methods may require knowledge of the morphologies beforehand to obtain structural parameters. In other words, for the complete characterization of the morphologies, one may need to know them first by the microscope and subsequently evaluate statistically the structural parameters by the scattering on the basis of the morphologies. Thus, the two methods have the pros and cons and are complementary to each other. According to the size of the morphologies, one may use an optical microscope together with light scattering (LS) for micron-scale morphologies and TEM (or SEM, AFM) with small-angle neutron (or X-ray) scattering for nanometer-scale structures. One of the biggest problems one might encounter in the course of the above conventional protocol is that the identification of complex structures by the microscopes is often inconclusive and hence interpretation of the scattering data would not be straightforward. The microscopes used so far are able to take two-dimensional (2D) (transmitted or surface) images of three-dimensional (3D) objects. The more complicated the morphologies are, the less convincing the interpretation of the 2D images usually become. It is thus requisite to develop microscopes that are capable of obtaining 3D images. Hereafter, we call such microscopes 3D microscopes and the methodology 3D-scopy or 3D microscopy. Due to these backgrounds, a couple of different types of 3D microscopes have been developed as described in Sect. 2. We emphasize that 3D microscopy should be accompanied by digital image analysis (see Sect. 3) that extracts useful and new structural information from the 3D volume data. In the present review, we will try to demonstrate that 3D microscopy has great advantages over the conventional methods to observe and analyze complex polymer structures. This review paper is organized in the following way. In Sect. 2, we briefly describe the basic principles of 3D microscopy that will be used later in this review paper. In Sect. 3, quantitative 3D image analysis for the 3D volume data on the basis of the geometry will be introduced. Section 4 is dedicated to the visualization of one of the transient

120

H. Jinnai et al.

structures observed in the polymer blend during the phase separation called spinodal decomposition (SD). It was found that the two domains form networks that coexist in 3D space (bicontinuous sructure). The stability of the interface between the two domains, the effects of preferential wetting and confinement on the SD process were examined using the (differential) geometry. 3D direct observation of the nanoscale structure of block copolymers will be discussed in terms of their stability in Sect. 5. The block copolymer morphology we dealt with exhibited bicontinuity similar to that of the one studied in the polymer blend. The effect of incorporation of the covalent bond (to form block copolymers) on the shape and regularity of the resulting morphologies is of particular interest, which will be discussed in Sect. 6. Finally, concluding remarks are given in Sect. 7.

2 3D Microscopy Figure 1 shows the spatial resolution of various types of microscopes and scattering methods. The figure includes 3D microscopy such as laser scanning confocal microscopy (LSCM), X-ray computerized tomography (X-ray CT), and transmission electron microtomography (TEMT). Although no experimental results obtained from the X-ray CT will be presented in the present review paper, we note that the microscopy [4] is particularly useful to

Fig. 1 Schematic illustration showing resolution of both microscopic and scattering methods. Abbreviations are the following: OM (optical microscopy), LSCM (laser scanning confocal microscopy), X-ray CT (X-ray computerized tomography), SEM (scanning electron microscopy), TEMT (transmission electron microtomography), ATF (atomic force microscopy), WAXS (wide-angle X-ray scattering), SAXS (small-angle X-ray scattering), LS (light scattering), USAXS (ultra-small-angle X-ray scattering), SANS (small-angle neutron scattering), and USANS (ultra-small-angle neutron scattering)

Emerging Technologies for the 3D Analysis of Polymer Structures

121

observe internal structures of opaque specimens. In the early 1990s, the spatial resolution of the X-ray CT was limited to ca. 100 m. Recently, a resolution comparable with that of the optical microscope (~1 m) has been achieved. It should be emphasized that, combining LSCM, X-ray CT, and TEMT, it is possible to establish a 3D microscopy whose resolution is over the wide range from nano- to micrometers. In what follows, we will briefly describe the principles and some applications for LSCM and TEMT. 2.1 Laser Scanning Confocal Microscopy (LSCM) After LSCM became commercially available in the late 1980s, the instrument generated an excitement among biologists. With LSCM, one can slice incredibly clean thin optical sections out of thick specimens, gain impressive 3D views at high resolution [5, 6]. The focal depth of the conventional optical microscopes is usually deep in comparison to its lateral resolution. This leads to the superposition of the out-of-focus images, and hinders the 3D interpretation of the images. Confocal microscopy has overcome this disadvantage by introducing a pinhole just in front of the detector as shown in Fig. 2. The solid line shows the opti-

Fig. 2 Optics of confocal microscopy. The incident light emitted from laser (1) is reflected by a dichroic mirror (2). The reflected light is focused on the specimen (4) through objective lens (3). At the focus the light may be reflected by the interior structure or the incident laser excites fluorescent molecules attached to the particular site (position) of the specimen. The reflected light or fluorescence from the focal plane refocuses at the confocal pinhole (5) and thus it passes the pinhole to reach detector (6). The out-of-focus light (fluorescence) is blocked by the confocal pinhole as shown by the dashed line

122

H. Jinnai et al.

cal path of reflected (or fluorescent) light in the focal plane of the objective lens. The reflected (or fluorescent) light focuses at the pinhole and reaches the detector. Simultaneously, the object may reflect the out-of-focus light (or emit the out-of-focus fluorescence), as shown by the dashed line in Fig. 2. In this case, simple ray tracing shows that the light (or fluorescence) reflected back to the confocal pinhole arrives as a defocused blur, only the central portion of which is detected and contributes to the image. In this way the system eliminates the images which do not lie within the focal region of the lens. The excellent depth resolution thus achieved, which is the full width at half maximum (fwhm) of optical sections, DF, is typically 1 m or may be less, depending on the optical setup. DF is a complicated function of an incident laser beam of wavelength, l, a numerical aperture (NA), magnification of the objective, radius of the confocal pinhole, refractive index of the object, etc. Once this “optical slicing” has been achieved, the objective (or the sample stage) is moved along the optical axis of the microscope to obtain a series of 2D optically sliced images, which is later used to reconstruct a 3D image (see Sect. 3.1 for details). To our best knowledge, Verhoogt et al. [7] first reported an application of LSCM to a polymer mixture. Although their work was instrument oriented and thus did not provide much insight into the phase-separated structure of the binary mixture itself, the potential of the instrument was clearly demonstrated. Image generation in LSCM of a polymer blend system was discussed by Ribbe et al. [8]. White and Wiltzius [9] discussed a mechanism of the phase separation in an off-critical polymer mixture through the time evolution of the size distribution of spherical domains. LSCM was applied to investigate the phase-separated structure of polymer mixtures at the critical composition, demonstrating that the structure is truly interconnected and periodically arranged, forming a 3D “maze” [10–12]. These studies are considered to take full advantage of 3D reconstruction intrinsic to LSCM. Morphology under a shear flow [13] and that of a ternary polymer mixture [14] were also studied by LSCM. We note that some other studies rather use the excellent depth resolution of the confocal microscope; surface and bulk structures of the solvent-cast films of a polymer mixture were investigated as a function of distance from the air–polymer surface [15, 16]. LSCM was also applied to investigate and demonstrate the penetration process of a spherulite into another spherulite of a different component in crystalline/crystalline polymer blends [17]. Besides those studies, LSCM was used for structural investigation of gel [18, 19], membrane systems [20, 21].

Emerging Technologies for the 3D Analysis of Polymer Structures

123

2.2 Transmission Electron Microtomography (TEMT) As already mentioned, TEMT is a method to image structures in 3D at nanometer-scale resolution [22]. Unlike confocal microscopy, TEMT uses a series of 2D projections taken by transmission electron microscopy (TEM) that are subsequently used to compute a 3D image of the object on the basis of computerized tomography (CT). TEMT offers a new approach to obtain 3D information of the order of the nanometer scale, and hence was rapidly developed during the past few years first in the biological community. Although the high potential of TEMT as a unique and powerful tool to study various types of structures in material science was recognized [23], it is only recently that the technique became available to the material community [24, 25]. So far, only a few studies [26–30] have used TEMT to investigate the complex 3D structures of polymeric materials, most of which dealt with the microphase-separated structures of block copolymers [see Sect. 5 for an example]. In what follows we will describe the principles of CT and subsequently discuss several experimental limitations in the TEMT measurements. The CT allows the complete 3D internal structure of an object to be reconstructed from a set of 2D projections at different angular settings, without imposing any a priori assumptions or requirements regarding the symmetry of the object. The reconstruction from projections is aided by an understanding of the relationship between an object and its projections in Fourier space: “the central slice theorem” [31] states that the Fourier transform of an objects projection is a central plane in the Fourier transform of the object as shown in Fig. 3. A projection of a 2D object, represented by the function f(x,y), is produced by parallel illumination from the electron source passing through the object, which is tilted at an angle j about an axis orthogonal to the beam path. p(r,j) denotes the projection in real space. The Fourier transform of p(r,j) is Z þ1 Fðq; jÞ ¼ pðr; jÞeiqr dr: ð1Þ 1

Here q is the wave number. The Fourier coefficients, F(q,f), are arranged along the line in Fourier space with the same tilting angle f. Gathering 2D projections over as wide a tilting range as possible gives a 3D Fourier transform of the object. Note that the ideal 180 range of tilt is required to give a complete sampling of Fourier space. Taking the inverse Fourier transform of the entire array of coefficients results in the reconstructed volume in real space. In the above 2D object case (in Fig. 3):

124

H. Jinnai et al.

Fig. 3 The discrete form of the central slice theorem in two dimensions. A projection p(r,j) in real space (x,y) at angle j is a slice F(q,j) at the same angle in Fourier space (qx,qy)

f ðx; yÞ ¼

2p Z þ1

Z 0

Fðq; jÞeiqðxcosjþysinjÞ qdqdj:

ð2Þ

0

Unfortunately the projection data are always sampled at discrete angles leaving regular gaps in Fourier space. The inverse Fourier transform intrinsically requires a continuous function, and therefore azimuthal interpolation is required to fill the gaps in Fourier space. The quality of the reconstruction is significantly affected by the type of interpolation implemented [32]. An alternative and more commonly used algorithm is the radius-weighted back projection technique [33]. In the case of TEMT, the projections at different angles are collected by tilting the specimen with respect to the electron beam in the TEM column. The tilt range achievable in a TEM is restricted by the relative geometries of specimen holder and objective lens since they will contact physically at high tilt angle, e.g., 70. The missing information due to this limitation becomes a wedge-shaped region of Fourier space, giving rise to a loss of resolution in the reconstructed image especially in the direction parallel to the electron beam. The restoration of the missing structural information has been studied intensively [34]. In addition, the resolution of the reconstructed image is strongly affected by the numbers of projections. The resolution is expressed as [35], r ¼ pDCT =NCT ;

ð3Þ

where r is the size of the smallest feature visualized in the reconstruction. DCT and NCT are the diameter (size) of the object or feature being reconstructed and the number of projections, respectively. Since the Fourier coefficients are radially arranged, more information will be lost as q increases, which limits the resolution of the reconstructed images. Equation 3 tells us that the resolution will be compensated by increasing the number of projec-

Emerging Technologies for the 3D Analysis of Polymer Structures

125

tions gathered; since NCT is increased, the density of the Fourier coefficients at a given q will be more dense. In reality, however, the angular increment in TEMT experiments is also limited to, at smallest, 1 (typically 2) due to the severe electron beam damage to the polymer specimens. During tilting the specimen, misalignments in the digitized images are also inevitable due to the imperfect eucentricity of the specimen stage. As a crucial prelude to calculating a 3D reconstruction, alignment of the digitized images is necessary. This is achieved either by least squares tracking of fiducial markers [22], such as small gold particles, or by sequential cross-correlation. Often a combination of both processes is used [36].

3 Digital Image Analysis of 3D Structures In the preceding section, two types of 3D microscopy were introduced. In some cases, it is sufficient to have 3D images of the structures in order to intuitively grasp their unique features. Actually, many researchers, in material science as well as in the medical and biological fields, seem to be content with 3D “pretty” pictures or the cross-sectional views of their 3D objects. This is merely “observations”, not “structural analysis”. Yet 3D microscopy gives much more structural information than either the conventional 2D microscopes or the scattering methods, most of which have never been acquired before. It is expected that the new structural information will clear up the root of unsolved physical problems. In the present section, we will introduce some quantitative analytical methods to extract such structural parameters from the 3D digital data. 3.1 3D Reconstruction In most cases, a 3D image is constructed from a stack of two-dimensional (2D) slices, i.e., a 3D array of image intensities. In the case of fluorescent LSCM, for example, the image intensities correspond to the concentration of fluorescent molecules that are chemically attached to one of the constituents. For quantitative image analysis, it is first necessary to isolate the portions of interest by defining surfaces that separate such particular parts from the other parts of the structures. The surfaces are called “interface”. One can assign the interface by specifying a threshold value for the image intensities. The marching cubes algorithm (MCA) [37] is used to find the interface from the 3D image. In this algorithm, a cube is created from the centers of eight adjacent pixels; four pixels from each of two adjacent slices. The image intensity at the pixels is assigned to the corresponding vertices of the cube. The interface is considered to intersect an edge of this cube if the in-

126

H. Jinnai et al.

tensity of one vertex of this edge is larger than the threshold value, and that of another vertex of the same edge is smaller than the threshold value. An intersecting point between the interface and the edge of the cube is determined by a linear interpolation according to the image intensity assigned to the two vertices on the edge. By properly connecting the intersections determined for the cube, the local interface is constructed and represented by a set of triangles. Note that the MCA defines the 14 types of intersection for the interface constructed in the cube by taking rotational and mirror symmetry into consideration (see Fig. 3 in ref. [37]). This gives a polygonal representation of the interface, which eventually reduces to triangles, from the 3D array of data by the MCA. A normal vector of each triangle, ntri, can be estimated by ntri ¼

ðp2 p1 Þ ðp3 p2 Þ ; jðp2 p1 Þ ðp3 p2 Þj

ð4Þ

where p1, p2, and p3 are the positional vectors of the vertices of the triangle. The normal vectors thus obtained from the MCA were used to evaluate normal vectors at vertices of the polygon, n. We note that the normal vectors obtained by the MCA, i.e., ntri, were those for the triangles comprising the polygon, not for the vertices. n was estimated by averaging the normal vectors of the neighboring triangles that shared the vertex of interest with those areas as a weighting: P i Si ntri : n ¼ i ð5Þ P Si ni tri i

Here nitri and Si denote, respectively, the normal vector and the area of the i-th neighboring triangle. Equation 5 will be further used to generate a parallel surface to measure surface curvatures (see Sect. 3.2.2 for details). 3.2 Curvature Distribution Measurements In some systems, the local shape of surfaces is significant in understanding the formation and stability of the morphologies and thus it can be a key structural measure to clarify the underlying physics. Surface curvatures are fundamental parameters characterizing the shape of surfaces in the differential geometry. From the volume data taken by the 3D microscopy, it is possible to determine the surface curvatures for the first time.

Emerging Technologies for the 3D Analysis of Polymer Structures

127

3.2.1 Surface Curvatures The curvatures at an arbitrary point on the surface can be expressed by two principal curvatures or the mean and Gaussian curvatures [38]. A 2D curvature is defined for a planar-curved path passing through a point of interest (POI) on the surface. The path is expressed by the intersection between the surface and the plane contains the surface normal vector at the point (see Fig. 4). Paths with different tangential directions on the surface have, in general, different values for the curvatures. Maximum and minimum values among those curvatures at the point of interest are called the principal curvatures, i.e., k1 and k2, as schematically shown in Figs. 4 and 7. Note that each curvature has a sign: it is positive if the path is convex from one side, negative otherwise, and zero if the path is straight. The mean curvature, H, and the Gaussian curvature, K, are defined as H¼

k1 þ k2 ; K ¼ k1 k2 : 2

ð6Þ

They are uniquely determined at the point p. The sign of K classifies the shape of the surface: it is elliptic if K>0, parabolic if K=0, and hyperbolic if K

Editorial Board: A. Abe · A.-C. Albertsson · R. Duncan · K. Dusek · W. H. de Jeu J. F. Joanny · H.-H. Kausch · S. Kobayashi · K.-S. Lee · L. Leibler T. E. Long · I. Manners · M. Mller · O. Nuyken · E. M. Terentjev B. Voit · G. Wegner

Advances in Polymer Science Recently Published and Forthcoming Volumes

Advanced Computer Simulation Approaches for Soft Matter Sciences I Volume Editors: Holm, C., Kremer, K. Vol. 173, 2004

Radiation Effects on Polymers for Biological Use Volume Editor: Kausch, H. Vol. 162, 2003

Microlithography · Molecular Imprinting Vol. 172, 2004

Polymers for Photonics Applications II Nonlinear Optical, Photorefractive and Two-Photon Absorption Polymers Volume Editor: Lee, K.-S. Vol. 161, 2003

Polymer Synthesis Vol. 171, 2004 NMR · Coordination Polymerization · Photopolymerization Vol. 170, 2004 Long-Term Properties of Polyolefins Volume Editor: Albertsson, A.-C. Vol. 169, 2004 Polymers and Light Volume Editor: Lippert, T. K. Vol. 168, 2004 New Synthetic Methods Vol. 167, 2004 Polyelectrolytes with Defined Molecular Architecture II Volume Editor: Schmidt, M. Vol. 166, 2004 Polyelectrolytes with Defined Molecular Architecture I Volume Editor: Schmidt, M. Vol. 165, 2004 Filler-Reinforced Elastomers · Scanning Force Microscopy Vol. 164, 2003 Liquid Chromatography · FTIR Microspectroscopy · Microwave Assisted Synthesis Vol. 163, 2003

Filled Elastomers · Drug Delivery Systems Vol. 160, 2002 Statistical, Gradient, Block and Graft Copolymers by Controlled/ Living Radical Polymerizations Authors: Davis, K.A., Matyjaszewski, K. Vol. 159, 2002 Polymers for Photonics Applications I Nonlinear Optical and Electroluminescence Polymers Volume Editor: Lee, K.-S. Vol. 158, 2002 Degradable Aliphatic Polyesters Volume Editor: Albertsson, A.-C. Vol. 157, 2001 Molecular Simulation · Fracture · Gel Theory Vol. 156, 2001 New Polymerization Techniques and Synthetic Methodologies Vol. 155, 2001 Polymer Physics and Engineering Vol. 154, 2001

NMR · 3D Analysis · Photopolymerization

With contributions by N. Fatkullin · T. Ikehara · H. Jinnai · S. Kawata · R. Kimmich T. Nishi · Y. Nishikawa · H.-B. Sun

The series presents critical reviews of the present and future trends in polymer and biopolymer science including chemistry, physical chemistry, physics and material science. It is addressed to all scientists at universities and in industry who wish to keep abreast of advances in the topics covered. As a rule, contributions are specially commissioned. The editors and publishers will, however, always be pleased to receive suggestions and supplementary information. Papers are accepted for “Advances in Polymer Science” in English. In references Advances in Polymer Science is abbreviated Adv Polym Sci and is cited as a journal. The electronic content of APS may be found at http://www.springerLink.com

ISSN 0065-3195 ISBN 3-540-20510-1 DOI 10.1007/b12766 Springer-Verlag Berlin Heidelberg New York

Library of Congress Control Number 2004105251 This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, re-printing, re-use of illustrations, recitation, broadcasting, reproduction on microfilms or in other ways, and storage in data banks. Duplication of this publication or parts thereof is only permitted under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer-Verlag. Violations are liable for prosecution under the German Copyright Law. Springer-Verlag is a part of Springer Science+Business Media springeronline.com Springer-Verlag Berlin Heidelberg 2004 Printed in Germany The use of registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting: Strtz AG, Wrzburg Cover: Knkellopka GmbH, Heidelberg; design&production GmbH, Heidelberg Printed on acid-free paper 02/3020/kk – 5 4 3 2 1 0

Editorial Board

Prof. Akihiro Abe

Prof. S. Kobayashi

Department of Industrial Chemistry Tokyo Institute of Polytechnics 1583 Iiyama, Atsugi-shi 243-02, Japan E-mail: [email protected]

Department of Materials Chemistry Graduate School of Engineering Kyoto University Kyoto 615-8510, Japan E-mail: [email protected]

Prof. A.-C. Albertsson Department of Polymer Technology The Royal Institute of Technology S-10044 Stockholm, Sweden E-mail: [email protected]

Prof. Ruth Duncan Welsh School of Pharmacy Cardiff University Redwood Building King Edward VII Avenue Cardiff CF 10 3XF United Kingdom E-mail: [email protected]

Prof. Karel Dusek Institute of Macromolecular Chemistry, Czech Academy of Sciences of the Czech Republic Heyrovsky´ Sq. 2 16206 Prague 6, Czech Republic E-mail: [email protected]

Prof. Dr. W. H. de Jeu FOM-Institute AMOLF Kruislaan 407 1098 SJ Amsterdam, The Netherlands E-mail: [email protected]

Prof. Prof. Kwang-Sup Lee Department of Polymer Science & Engineering Hannam University 133 Ojung-Dong Taejon 300-791, Korea E-mail: [email protected]

Prof. L. Leibler Matire Molle et Chimie Ecole Suprieure de Physique et Chimie Industrielles (ESPCI) 10 rue Vauquelin 75231 Paris Cedex 05, France E-mail: [email protected]

Prof. Timothy E. Long Department of Chemistry and Research Institute Virginia Tech 2110 Hahn Hall (0344) Blacksburg, VA 24061, USA E-mail: [email protected]

Prof. Ian Manners Department of Chemistry University of Toronto 80 St. George St. M5S 3H6 Ontario, Canada E-mail: [email protected]

Prof. Jean-Franois Joanny Institute Charles Sadron 6, rue Boussingault F-67083 Strasbourg Cedex, France E-mail: [email protected]

Prof. Hans-Henning Kausch c/o IGC I, Lab. of Polyelectrolytes and Biomacromolecules EPFL-Ecublens CH-1015 Lausanne, Switzerland E-mail: [email protected]

Prof. Dr. Martin Mller Deutsches Wollforschungsinstitut an der RWTH Aachen e.V. Veltmanplatz 8 52062 Aachen, Germany E-mail: [email protected]

Prof. Oskar Nuyken Lehrstuhl fr Makromolekulare Stoffe TU Mnchen Lichtenbergstr. 4 85747 Garching, Germany E-mail: [email protected]

VI

Editorial Bord

Dr. E. M. Terentjev

Prof. Gerhard Wegner

Cavendish Laboratory Madingley Road Cambridge CB 3 OHE United Kingdom E-mail: [email protected]

Max-Planck-Institut fr Polymerforschung Ackermannweg 10 Postfach 3148 55128 Mainz, Germany E-mail: [email protected]

Prof. Brigitte Voit Institut fr Polymerforschung Dresden Hohe Straße 6 01069 Dresden, Germany E-mail: [email protected]

Advances in Polymer Science Also Available Electronically

For all customers who have a standing order to Advances in Polymer Science, we offer the electronic version via SpringerLink free of charge. Please contact your librarian who can receive a password for free access to the full articles by registering at: http://www.springerlink.com If you do not have a subscription, you can still view the tables of contents of the volumes and the abstract of each article by going to the SpringerLink Homepage, clicking on “Browse by Online Libraries”, then “Chemical Sciences”, and finally choose Advances in Polymer Science. You will find information about the – Editorial Board – Aims and Scope – Instructions for Authors – Sample Contribution at http://www.springeronline.com using the search function.

Contents

Polymer Chain Dynamics and NMR R. Kimmich · N. Fatkullin . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

1

Emerging Technologies for the 3D Analysis of Polymer Structures H. Jinnai · Y. Nishikawa · T. Ikehara · T. Nishi . . . . . . . . . . . . . . . . . . . . . . 115 Two-Photon Photopolymerization and 3D Lithographic Microfabrication H.-B. Sun · S. Kawata . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 169 Author Index Volumes 101–170 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 275 Subject Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 291

APS (2004) Single Contribution:1--113 DOI 10.1007/b12766 Springer-Verlag 2004

Polymer Chain Dynamics and NMR Rainer Kimmich1 (*) · Nail Fatkullin2 1

Sektion Kernresonanzspektroskopie, Universitt Ulm, 89069 Ulm, Germany [email protected] 2 Department of Molecular Physics, Kazan State University, 420008 Kazan, Tatarstan, Russia

1

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

2 NMR Methods . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 NMR Diffusometry. . . . . . . . . . . . . . . . . . . . . . . 2.1.1 Hahn Spin Echo in the Short Gradient Pulse Limit (dD) . 2.1.1.1 Gaussian Propagators . . . . . . . . . . . . . . . . . . . . . 2.1.1.2 Non-Gaussian Propagators . . . . . . . . . . . . . . . . . . 2.1.2 Hahn Spin Echo for Long Gradient Pulses . . . . . . . . . . 2.1.3 Stimulated Echo . . . . . . . . . . . . . . . . . . . . . . . . 2.1.4 Spin Echoes and Steady B0 Gradients. . . . . . . . . . . . . 2.2 NMR Spin–Lattice Relaxometry. . . . . . . . . . . . . . . . 2.2.1 General Theoretical Background . . . . . . . . . . . . . . . 2.2.2 The Field-Cycling NMR Relaxometry Technique . . . . . . 2.3 Residual Dipolar Broadening and Transverse Relaxation . . 2.3.1 The Anderson/Weiss Approach . . . . . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

5 6 6 8 9 10 10 11 13 14 17 20 21

3 Modeling of Chain Dynamics and Predictions for NMR Measurands 3.1 The Rouse Model. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1.1 Translational Segment Diffusion of a Rouse Chain . . . . . . . . . . . 3.1.2 Spin–Lattice Relaxation of a Rouse Chain . . . . . . . . . . . . . . . . 3.2 The Tube/Reptation Model . . . . . . . . . . . . . . . . . . . . . . . . 3.2.1 The Doi/Edwards Limits . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2.2 Echo Attenuation by Reptation . . . . . . . . . . . . . . . . . . . . . . 3.2.3 General Remarks on the Tube/Reptation Model . . . . . . . . . . . . . 3.3 Memory Function Formalisms . . . . . . . . . . . . . . . . . . . . . . 3.3.1 The Generalized Langevin Equation (GLE) . . . . . . . . . . . . . . . 3.3.2 The GLE for the Tagged Macromolecule . . . . . . . . . . . . . . . . . 3.3.2.1 The Potential of the Mean Force and the Memory Matrix . . . . . . . 3.3.2.2 The Rouse Equation of Motion as a Special Case of the GLE . . . . . . 3.4 Renormalized Rouse Models . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 The First Renormalization. . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 The Second Renormalization . . . . . . . . . . . . . . . . . . . . . . . 3.4.3 General Remarks on Renormalized Rouse Models . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

22 24 27 28 29 30 34 35 37 37 39 42 43 45 47 51 55

Experimental Studies of Bulk Melts, Networks and Concentrated Solutions. The Three Components of Polymer Dynamics as Relevant for NMR Relaxometry . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Component A. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Component B . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Component C . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Different Time-scale Approach for the NMR Correlation Function . . . .

57

4 4.1 4.1.1 4.1.2 4.1.3 4.1.4

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

3

57 58 60 61 61

2

R. Kimmich · N. Fatkullin

4.1.5 Average Transverse Relaxation . . . . . . . . . . . . . . . . . . . . . 4.1.5.1 Characteristic Temperature . . . . . . . . . . . . . . . . . . . . . . . 4.1.5.2 Characteristic Molecular Weights . . . . . . . . . . . . . . . . . . . . 4.1.5.3 Crossover from the Melt to Dilute Solutions . . . . . . . . . . . . . . 4.2 Chain-end Dynamics (“Whip Model”) . . . . . . . . . . . . . . . . . 4.3 Free-Volume and Void Effects . . . . . . . . . . . . . . . . . . . . . . 4.4 Evidence for Rouse Dynamics (M<Mc). . . . . . . . . . . . . . . . . 4.5 The Three Regimes of Spin–Lattice Relaxation Dispersion in Entangled Polymer Melts, Solutions, and Networks (M<Mc) . . . 4.5.1 High- and Low-Mode-Number Limits (Dispersion Regions I and II) 4.5.2 Intra- and InterSegment Spin Interactions (Dispersion Region III) . 4.5.3 Mesomorphic Phases . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5.4 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5.5 Networks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.6 Translational Segment Diffusion and Spin Diffusion . . . . . . . . . 4.6.1 Center-of-Mass Diffusion . . . . . . . . . . . . . . . . . . . . . . . . 4.6.2 Anomalous Segment Diffusion . . . . . . . . . . . . . . . . . . . . . 4.6.3 Flip-Flop Spin Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . .

. . . .

. . . .

. . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

62 65 68 70 71 75 76

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

79 85 87 92 95 96 97 97 99 100

. . . .

. . . .

. . . .

. . . .

5 5.1 5.2 5.3

Chain Dynamics in Pores (“Artificial Tubes”) . . . . . . . Diffusion in Pores . . . . . . . . . . . . . . . . . . . . . . . Spin–Lattice Relaxation Dispersion in Pores. . . . . . . . . Theoretical Crossover from Rouse to Reptation Dynamics .

. . . .

101 103 104 105

6

Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

107

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

109

Abstract The universal features of polymer dynamics are specifically represented by laws for (anomalous) segment diffusion and chain relaxation modes. Nuclear magnetic resonance (NMR)-based techniques provide direct access to these phenomena. This in particular refers to NMR relaxation and diffusion studies. Methods suitable for this purpose are described in detail. Three basic classes of polymer dynamics models, namely the Rouse model, the tube/reptation model, and the renormalized Rouse models are outlined and discussed with respect to predictions for NMR measurands. A wealth of experimental NMR data are reviewed and compared with predictions of the model theories. It is shown that characteristic features of all three types of models can be verified in great detail provided that the model premisses are suitably mimicked in the experiments. Rouse dynamics is shown to be relevant for polymer melts with molecular weights below the critical value and for solutions of diminished entanglement effect. Features specific for the renormalized Rouse model reveal themselves in the form of high- and low-mode-number limits of the spin–lattice relaxation dispersion. These results are considered to mirror the analytical structure of the Generalized Langevin Equation. Finally, anomalous-diffusion and relaxation laws characteristic for the tube/reptation model can be perfectly reproduced in experiment if the polymer chains are confined in a nanoporous, solid matrix whereas bulk melts are not in accord with these predictions. The dynamics of chains confined in artificial tubes can be treated analytically assuming a harmonic radial potential for the polymer/wall interaction. These results derived for a real tube closely render the characteristic features of the original Doi/Edwards model predicted for a fictitious tube.

Polymer Chain Dynamics and NMR

3

Keywords NMR · Relaxation · Diffusion · Rouse model · Reptation · Renormalized Rouse model Abbreviations BWR CLF CPMG FID GLE NMR ODF PB PDES PDMS PE PEO PGSE PHEMA PIB PIP PMMC PS PTHF PU RF RRM SGSE ThRRM TRRM WLF

Bloch/Wangsness/Redfield theory contour length fluctuation Carr/Purcell/Meiboom/Gill free-induction decay generalized Langevin equation nuclear magnetic resonance order director fluctuations poly(butadiene) poly(diethylsiloxane) poly(dimethylsiloxane) poly(ethylene) poly(ethylene oxide) pulsed gradient spin echo method poly(hydroxyethylmethacrylate) poly(isobutylene) poly(isoprene) polymer mode-mode coupling model poly(styrene) poly(tetrahydrofurane) phenylurazole radio frequency renormalized Rouse model steady gradient spin echo method three times renormalized Rouse model twice renormalized Rouse model Williams/Landel/Ferry

1 Introduction The objective of this review is to outline the basic theories and models of linear polymer chain dynamics [1], and to demonstrate the potential of NMR (nuclear magnetic resonance) techniques for probing the characteristics of molecular motions in such systems. From the methodological point of view we will mainly focus on field-cycling NMR relaxometry and fieldgradient NMR diffusometry, but will also make some reference to transverse relaxation and the residual dipolar interaction occurring in entangled polymer systems. This combination of methods turned out to be most powerful for the examination of chain modes and the translational diffusion properties of polymer segments and the coil center-of-mass. The techniques referred to are best suited to shed light on almost every aspect of polymer dynamics.

4

R. Kimmich · N. Fatkullin

Particular emphasis will be laid on the experimental verification of features of standard theories of polymer dynamics such as the Rouse model, the tube/reptation model [1] or the renormalized Rouse models. Based on the special conditions under which predictions of these theories match experimental findings well, the application limits and the deficiencies of these models for more general scenarios become obvious and help to ameliorate the underlying model ansatz for chain dynamics. In order to elucidate the universal character of polymer chain dynamics, we will attempt to consider as many different polymer species as possible for which NMR relaxometry and diffusometry data are available. On the other hand this means that we must restrict ourselves predominantly to melts of linear homopolymers with a narrow molecular weight distribution to keep the range of literature referred to at manageable levels. Only where enlightening information is expected will we refer to solutions, networks, and mesomorphic systems in addition to isotropic melts. Empirically the conclusions suggested by the huge amount of experimental NMR data available in the literature provide a complete picture rendering dynamical features in great detail. This is in contrast to the stage of development of model theories where the “many-entangled-excluded-volume-chain” problem still has to be overcome, although promising approaches exist. In particular it will turn out that the theoretical concepts available for this sort of system are unable to describe many experimental details quantitatively. On the other hand, predictions of all model theories referred to in this context will be shown to be compatible with certain experimental findings provided that the sample and measuring conditions are adapted to the scenarios that were anticipated in the theoretical derivations. Apart from the introductory section, the article is subdivided into four major sections: NMR Methods; Modeling of Chain Dynamics and Predictions for NMR Measurands; Experimental Studies of Bulk Melts, Networks, and Concentrated Solutions; and Chain Dynamics in Pores. First, the NMR techniques of interest in this context will be described. Second, the three fundamental polymer dynamics theories, namely the Rouse model, the tube/reptation model, and the renormalized Rouse theories are considered. The immense experimental NMR data available in the literature will be classified and described in the next section, where reference will be made to the model theories wherever possible. Finally, recent experiments, analytical treatments, and Monte Carlo simulations of polymer chains confined in pores mimicking the basic premiss of the tube/reptation model are discussed.

Polymer Chain Dynamics and NMR

5

2 NMR Methods NMR provides a rich variety of methods for polymer studies. This in particular refers to the chemical structure of such compounds. Here we deliberately restrict ourselves to investigations on length scales, where chemical bonds and interactions merely matter indirectly via parameters such as segment lengths or friction coefficients. That is, we are dealing with dynamic properties of Kuhn segment chains for times or frequencies beyond those relevant for fluctuations within Kuhn segments. Any chemical shift-based spectroscopy is beyond the scope of this review. Figure 1 shows a schematic representation of the fluctuation time or angular frequency ranges covered by the methods of interest in this context. We will be referring mainly to field-cycling NMR relaxometry combined with conventional high-field methods, to field-gradient NMR diffusometry, and, to a minor degree, to dipolar broadening-based techniques such as the dipolar correlation effect. For an introduction to these methods the reader is referred to monographs like Ref. [2]. Diffusion in polymers can manifest itself in “normal” or “anomalous” form depending on the time or displacement length scale probed in the experiment. The criterion for this distinction is the time dependence of the mean squared displacement 2 k R /t ð1Þ valid in the form of a power law in random unrestricted media. An exponent k=1 indicates normal diffusion as is expected for center-of-mass diffusion, i.e., root mean square displacements much larger than the Flory radius. On the other hand, k> te=tsNe2, where NeNc/2. Intermolecular entanglement forces effectively localize the macromolecule in a space region in the form of a curved tube of diameter d=bNe around the contour line or primitive path of the chain (see Fig. 7). The tube conformation corresponds to that of a freely jointed chain, that is, the tube conformation has a Gaussian end-to-end length distribution. The characteristic time 1 te ts Ne2 ts Nc2 4

ð65Þ

is called the entanglement time, and Ne is the number of Kuhn segments effectively corresponding to an “entanglement”. Segments moving inside the tube are considered to move in a viscous medium as it is anticipated in the Rouse model. In the interior of the tube, entanglement interactions are assumed to be absent. However, as soon as a segment approaches the tube “walls”, entanglement forces become infinitely large so that the polymer is effectively confined by the topological constraints imposed by the tube. The chain-end segments are excepted from this restraint: they are not subject to entanglement forces and can therefore move isotropically. The consequence is that the chain can migrate in a reptile manner (reptation) into a new conformation completely uncorrelated to that of the initial chain coil. 3.2.1 The Doi/Edwards Limits There are four dynamic processes characterized by the four characteristic time constants of the tube/reptation model (see Fig. 7): the segment fluctuation time ts (given in Eq. 53), the entanglement time te (given in Eq. 65), the (longest) Rouse relaxation time tR (given in Eq. 54), and the (tube) disengagement time td (given below in Eq. 71). With these four time constants, four dynamic limits can be defined, which will be termed the Doi/Edwards limits (I)DE to (IV)DE. Table 1 shows the limiting laws for the mean squared

Polymer Chain Dynamics and NMR

31

Fig. 7. Illustration of a polymer chain (the tagged chain) confined in the fictitious tube of diameter d formed by the matrix. The contour line of the tube is called the primitive path having a random-walk conformation with a step length a=d. The four characteristic types of dynamic processes (dotted arrow lines) and their time constants ts, te, tR, and td defined in the frame of the Doi/Edwards tube/reptation model are indicated

segment displacement and the spin–lattice relaxation time commonly expected on this basis. Figure 7 illustrates the chain processes dominating in the four limits. Limit (I)DE (ts >N, the time dependence of the normal mode relaxation functions can be approximated by an exponential decay as t : ð130Þ Cp ðt Þ ¼ Cp ð0Þ exp tp Otherwise Eq. 117 can be solved only numerically. It was found, that the solution of the equation can be approximated by the stretched exponential (Fig. 10) ( ) t bp Cp ðt Þ Cp ð0Þ exp ; ð131Þ ~tp

Fig. 10. Numerically evaluated, normalized autocorrelation function for the RRM for p=5 together with a fitted curve for a stretched exponential, Eq. 131, and an exponential curve. The stretched-exponential parameter is b5=0.66

50

R. Kimmich · N. Fatkullin

Fig. 11. Mode number dependence of the stretching-parameter bp for the RRM (see Eq. 131) for different entanglement parameters y. The number of Kuhn segments was assumed to be N=100 b

p t and bp is a mode-number-dependent stretching parameðbp Þ p ter (see Fig. 11). G(bp) is the gamma function. In the same limit, the mean squared segment displacement obeys ( 2=5 2 t 2 0:23b for t tRR ~ 1 ; yts Rn ðt Þ ¼ ð132Þ 6DRR t for t tRR 1

where ~tp ¼ G

where DRR ¼

0:21 b2 3p2 yts N 3=2

ð133Þ

is the center-of-mass diffusion coefficient in the RRM. The correlation function of the segment tangent vector calculated in the Markovian approximation is in the low-mode-number limit given by 8 D E < b2 yts 2=5 for t tRR 1 ~ bn ðt Þ ~ bn ð0Þ ’ b2 t n t o : ð134Þ RR : N exp RR for t t1 t 1

These results should be asymptotically correct in the limit N!1 and t >> 0.05(6p)4yts. For finite N, the exponents predicted in Eq. 132 may change slightly due to the stretched exponential decay of Cp(t) given in Eq. 131. The limiting laws for the observables of interest in the frame of this review, the mean squared displacement and the (intrasegment) spin–lattice relaxation rate, are summarized in Table 2 (compare [49]).

Polymer Chain Dynamics and NMR

51

Table 2. Theoretical dependences on time (t), angular frequency (w), molecular mass (M), or number of Kuhn segments (N) predicted by the (once) renormalized Rouse model for the mean squared segment displacement and the intrasegment spin–lattice relaxation time. The factors CI, CIRR, CIIRR, and CIIIRR are frequency and molecular mass independent constants Limit

Rouse

(I)RR

(II)RR

ts > < w0 0:730:05 Mw w (region I ‘‘mesophase’’) T1 / : ð182Þ 0 0:250:05 M w (region II ‘‘isotropic phase’’) > > : w0 0:450:05 (region II ‘‘mesophase’’) Mw w

Polymer Chain Dynamics and NMR

93

The slopes in region II for both the isotropic and the mesomorphic phases are in accordance with data for the spin–lattice relaxation time in the rotating frame, T1p. These results for the ordered mesophase are to be compared with the spin–lattice relaxation dispersion expected for nematic liquid crystals where a power law T1 / n0:5 ðODFÞ

ð183Þ

is predicted for order director fluctuations (ODF) at low frequencies [161– 167]. With nematic compounds this law and the collective fluctuations in the ordered state it represents should show up irrespective of whether it is a monomeric or polymeric substance. This is in contrast to the mesophase of PDES. The monomers of this compound do not show any order because they do not contain mesogenic groups. That is, the order observed in the PDES mesophase must have a thermodynamic background different from that of nematic phases. It is concluded that the modified power laws for spin–lattice relaxation dispersion in the mesophase reflect a modified behavior of chain modes rather than collective fluctuations of ensembles of molecules in ordered domains. This conclusion is corroborated by the identical frequency dispersion of the spin–lattice relaxation times T1 and T1p in the laboratory and in the rotating frames, respectively. If the order in the PDES mesophase would be of a nematic nature and the fluctuations causing dispersion region II consequently would be of the ODF type, the frequency dispersion of T1p should vanish while that of T1 is retained [22]. In this context, a study of the dipolar correlation effect in the mesophase of PDES is of particular interest [168]. Using this technique, it was concluded that the sample consists of defect-enriched areas and ordered domains. The two dynamic states are connected with segments of different mobility, and they fluctuate temporally and spatially. The exchange times between the two mobility states range between 0.1 and 1.0 s in the mesomorphic temperature range. The exchange process between the two environments is slow compared with the transverse relaxation rates so that the two signal components can clearly be distinguished. This is in contrast to spin–lattice relaxation where flip-flop spin diffusion as an additional exchange mechanism mediates averaging over all heterogeneities. Spin–lattice relaxation curves therefore decay mono-exponentially in a wide range [155], whereas the transverse magnetization is subject to a superposition of virtually two exponential functions [168]. As concerns the different power law regimes of spin–lattice relaxation given in Eq. 182, it is not yet known to which of the two segment phases they must be attributed or to what degree exchange averaging matters in this respect.

94

R. Kimmich · N. Fatkullin

Fig. 39. Fraction of the more mobile segments in the mesophase of polydiethylsiloxane (PDES) as a function of the reduced temperature. The solid line represents Eq. 184

The dipolar correlation effect is based on stimulated-echo signals [2] and therefore contains elements both of transverse and longitudinal relaxation. Flip-flop spin diffusion as well as material transport may contribute to the exchange mechanism identified this way. An interesting result of the dipolar correlation effect study is the temperature dependence of the fraction of the more mobile segments which was shown to obey the empirical law (see Fig. 39) [168] T Tc Pa ¼ exp 45 ; ð184Þ T where Tc is the (molecular weight dependent) isotropization temperature. Approaching Tc from below increases the fraction of the more mobile segments exponentially as a function of the reduced temperature. Figure 40 shows an attempt to visualize how the areas of different mobility could arise based on “collapsed” coils. The “gain” in chain mobility in the ordered mesophase is attributed to conformations containing many chain folds compensating the dynamic restrictions entailing the almost nematiclike order in this phase (compare the discussion in context with chain-end dynamics and the statistical physics treatment of chain folds in Ref. [124]).

Polymer Chain Dynamics and NMR

95

Fig. 40. Attempt to schematically represent the ordered mesophase of PDES juxtaposed to the isotropic phase. The “collapsed” coil structure assumed in the mesophase entails chain folds that provide additional motional degrees of freedom and is therefore thermodynamically stabilized in a certain temperature range (compare the statistical physics treatment in Ref. [124]). The shaded ellipses indicate somewhat closer packed, more ordered and less mobile areas in contrast to the more mobile, more distorted chain conformations in regions where many folds accumulate

4.5.4 Solutions The features of entangled polymer dynamics fade upon dilution by a lowmolecular solvent. In other words, the critical molecular weight characteristic for the crossover between Rouse-like and entangled dynamics is growing with the degree of dilution (see Eq. 162). NMR relaxation measurements turned out to be particularly suitable for studies of the dilution process. The crossover from the melt to the dilute solution was already demonstrated with the T2/T1 ratio in Fig. 20. It can also be visualized with the aid of spin– lattice relaxation dispersion of PDMS dissolved in CCl4 as a proton-free solvent. Figure 31d shows corresponding data. Compared to the region II dispersion occurring as one of the characteristics of melts of entangled polymers the spin–lattice relaxation dispersion becomes flatter upon dilution. With a PDMS content of 15% in CCl4 the data can be described by the Rouse model as the incarnation of free-chain dynamics (see Fig. 31d). This may appear surprising since the critical molecular weight for this concentration according to Eq. 162 is below the weightaverage molecular weight of the polymer examined, Mw=423,000, so that entangled dynamics should still apply. On the other hand, all polymer dynamics models unspecifically predict some short-time/high-frequency limit where Rouse-like behavior should dominate (see Tables 1–3). In melts of entangled polymers such a regime could never be identified by spin–lattice relaxation dispersion because component B in the form of the high-mode-number limit (region I) appears to overlap with the local segment fluctuation regime (manifesting itself as com-

96

R. Kimmich · N. Fatkullin

ponent A). That is, there is no intermediate time or frequency window left in entangled melts where Rouse dynamics could develop in full. Such a dynamic gap obviously arises in solutions if the polymer concentration is low enough. Component A representing local segment fluctuations becomes accelerated upon dilution, whereas the entanglement effect on the chain modes is shifted to correspondingly longer length and time scales. That is, a very important theoretical requirement is satisfied in this way. We will come back to the topological constraint problem later in the review. 4.5.5 Networks Permanent or thermoreversible cross-links mediate the opposite effect on chain dynamics compared with dilution by a solvent: instead of releasing topological constraints by dilution, additional hindrances to chain modes are established by the network. With respect to NMR measurands relatively large cross-link densities are needed to affect chain modes visible in the experimental time/frequency window, as demonstrated with proton spin–lattice relaxation dispersion of polyethylene cross-linked by 10-Mrad irradiation with electron beams [123] and with styrene–butadiene rubbers [29]. However, there is a very strong effect on the dipolar correlation effect which probes much slower motions and can therefore be used favorably for the determination of the cross-link density [29, 176, 177]. In the plot shown in Fig. 31e, spin–lattice relaxation dispersion curves of permanently cross-linked PDMS are shown. With decreasing mesh length, the chain modes appear to be shifted to lower frequencies. This is indicated by lower values of the relaxation times while the dispersion slopes of regions I and II are retained. On the other hand, the effect on the crossover frequency is minor. The fact that the dispersion regions I, II, and III of proton spin–lattice relaxation retain their qualitative appearance in the presence of (in this case thermoreversible) cross-links is demonstrated in Fig. 34. The influence of fluctuating cross-links on the dispersion curves can be explained by an effectively modified monomeric friction coefficient [131]. A result of particular interest is the shift of the crossover frequencies between dispersion regions I, II, and III. The shifts can be explained by the ratios nI;II nII;III ~ts ¼ ¼ ; ~nI;II ~nII;III ts

ð185Þ

where the quantities with tilde refer to networks. The friction effect on segment fluctuations equally slows down chain modes at the lowest frequencies.

Polymer Chain Dynamics and NMR

97

4.6 Translational Segment Diffusion and Spin Diffusion The NMR diffusometry techniques described in this article are frequently and suitably used for tests of the limits for the mean squared segment displacement predicted by polymer theories. The time and length scales probed by the techniques can be adjusted by the corresponding pulse intervals and the field gradient strength (the “wave number”), respectively. In this way, one gets access to the center-of-mass diffusion limit as well as to the anomalous-segment diffusion regime. The root mean squared displacements examined in the former case are larger than the coil dimension, whereas the latter limit is probed if the displacements are shorter than the coil extension. 4.6.1 Center-of-Mass Diffusion NMR diffusometry is suitable for studies of the center-of-mass diffusion coefficient provided that the diffusion time can be chosen longer than the terminal relaxation time. In terms of the tube/reptation model, this is limit (IV)DE defined by t>>td. Eq. 75 suggests D/Mw2.0 which appears to have been verified several times in experiment [8, 148–150, 169–171]. Figure 41 shows polydimethylsiloxane melt data as a typical example [8]. Data for other polymer melt examples reported in the literature refer to polystyrene and polyethylene at different temperatures [169, 148, 149], and polyethyleneoxide [11, 170]. It appears that all those data perfectly corroborate the validity of limit (IV)DE of the tube/reptation model. However, there are four reasons why the molecular weight dependence observed in experiments may be modified by factors other than the tube constraints: – The condition t>>td is difficult to achieve with high molecular weights so that the anomalous segment displacement regime may gain an increasing influence from low to high molecular weights, as was clearly demonstrated at least with the two highest molecular weights in the plot shown in Fig. 41 [8]. The consequence is an apparently weaker molecular weight dependence. The crossover regime between the center-of-mass and the anomalous segment displacement regimes was extensively studied [172] for polystyrene solutions. It appears that the center-of-mass diffusion coefficient cannot be evaluated reliably by the field-gradient technique without considering the crossover to the anomalous diffusion regime at the same time. – Free volume connected with chain-end blocks influences the molecular weight dependence of chain dynamics in the vicinity of Mc. An apparently steeper molecular weight dependence results on these grounds particularly below Mc. The failure of NMR techniques to directly render the molecular

98

R. Kimmich · N. Fatkullin

Fig. 41. Center-of-mass diffusion coefficient in polydimethylsiloxane (PDMS) melts at 20.5 C [8] as a function of the molecular weight. This self-diffusion coefficient is relevant for root mean square displacements exceeding the random-coil dimension. The experimental condition is that the echo attenuation is recorded with small field-gradient strengths and correspondingly long diffusion times. The straight line represents the law D/Mw2 which seemingly coincides with the prediction by the tube/reptation model for limit (IV)DE (see Eq. 75). The deviation from the Mw2 dependence above Mw=100,000 is due to the fact that in this case the diffusion time could not be chosen long enough to ensure center-of-mass diffusion. Actually we are here already in the anomalous segment diffusion regime. For Mw=250,000, for instance, the root mean square displacement reached along the gradient direction in a diffusion time of 30 ms is only 20 nm compared with a radius of gyration of 25 nm

weight dependence D/Mw1.0 predicted for the Rouse model (see Eq. 59) was explained in this way [148, 149]. – At very high molecular weights, when the diffusion coefficient due to flipflop spin diffusion of the order 1015 m2/s is getting comparable to the ordinary Brownian self-diffusion coefficient, a flatter chain length dependence of the effective diffusion coefficient is expected [10].

Polymer Chain Dynamics and NMR

99

– If very broad, the molecular weight distribution may influence the (average) center-of-mass diffusion coefficient evaluated from echo attenuation curves [169, 175].

In view of the contour-length fluctuation mechanism suggested by Doi as an explanation of the fractional exponent of the power law for the zero-shear viscosity [142], h/Mw3.4, a molecular weight dependence somewhat stronger than predicted by Eq. 75 was predicted also for the center-of-mass diffusion coefficient [169]. More recent studies mainly carried out with concentrated solutions even suggest power laws with universally stronger molecular weight dependences than predicted by the tube/reptation model [172–174]: D / Mw2:40:1 f1:80:2 ; h / Mw3:40:1 f3:80:2 ;

ð186Þ

where f is the volume fraction of the polymer. 4.6.2 Anomalous Segment Diffusion Because of the relatively short displacement time or length scales typically probed by NMR diffusometry, it is particularly well suited to detect anomalies in the segment displacement behavior expected on a time scale shorter than the terminal relaxation time, that is for root mean squared displacements shorter than the random-coil dimension. All models discussed above unanimously predict such anomalies (see Tables 1–3). Therefore, considering exponents of anomalous mean squared displacement laws alone does not provide decisive answers. In order to obtain a consistent and objective picture, it is rather crucial to make sure that (i) the absolute values of the mean squared segment displacement or the time-dependent diffusion coefficient are compatible with the theory, (ii) the dependence on other experimental parameters such as the molecular weight are correctly rendered, and (iii) the values of the limiting time constants are not at variance with those derived from other techniques. For instance, the segmental friction coefficient or the mean squared endto-end distance can be determined directly from viscoelasticity or neutron scattering data. Estimating segment diffusion with the aid of the tube/reptation model based on such data leads to unrealistic predictions. The predicted segment displacements tend to be much too large [9, 12, 178]. Figure 42 shows polyethyleneoxide data as an example. One identifies a time dependence D(t)/t0.5 at short diffusion times in contrast to the law D(t)/t3/4 predicted for te 0.1 s is due to flip-flop spin diffusion which physically limits the detection of molecular displacements by NMR diffusometry

(compare Fig. 44) using the formalism specifically derived for the tube/reptation model (see Eqs. 76–79). In the frame of the experimental accuracy, it is not possible to describe the whole family of echo attenuation curves on the basis of the unmodified predictions in the full diffusion time range for all molecular weights at the same time [9, 12, 178], even if flip-flop spin diffusion (see the following section) is taken into account. On the other hand, if a static “tube” really exists as anticipated in the tube/reptation model, the predictions for anomalous segment diffusion are adequate, of course, and can be verified in experiment. This will be demonstrated by considering linear polymers confined in nanopores. 4.6.3 Flip-Flop Spin Diffusion Flip-flop spin diffusion is a phenomenon specific for NMR. It does not matter with other techniques. Spin diffusion based on Zeeman energy conserving flip-flop transitions of dipolar coupled spins, that is interchange of spin-

Polymer Chain Dynamics and NMR

101

up and spin-down states, is normally negligible compared to molecular selfdiffusion in liquids. However, with viscous systems with little motional averaging of dipolar coupling and with the aid of very strong field gradients, NMR diffusometry is able to detect this immaterial transport mechanism competing with molecular diffusion. Spin echoes can be attenuated on this basis just as with any other incoherent displacement process [181]. Employing the strong fringe-field gradient of a superconducting magnet, it was possible to demonstrate the influence of flip-flop spin diffusion on the echo attenuation of polymer melts [10, 12]. The experiments were carried out by diluting the polymer under investigation isotopically. That is, undeuterated polymers were dissolved in a perdeuterated matrix of polymers of equivalent molecular weight. The reduction of intermolecular dipolar interactions diminishes the proton spin flip-flop rate as expected. The effect is also evident in Fig. 42 referring to a polyethyleneoxide melt with an extremely large molecular weight, Mw=5,000,000. The time-dependent diffusion coefficient was evaluated in the low wave number approximation, Eq. 27, according to hR2(t)i=6D(t)t. The time-independent plateau appearing at times t >> 0.1 s was shown to be due to flip-flop spin diffusion [10, 12]. As a consequence, the proper evaluation of segment diffusion at long diffusion times turned out to be more complicated than often anticipated. However, even with flip-flop spin diffusion theoretically taken into account, it is not possible to fit the formulas predicted by the tube/reptation model to the experimental data with respect to both the time and molecular weight dependences in a consistent way and without assuming unrealistic parameters [12].

5 Chain Dynamics in Pores (“Artificial Tubes”) The motivation to study the dynamics of polymer chains confined in nanoporous materials with more or less rigid pore walls is twofold. Firstly, there may be important technological applications requiring knowledge on the dynamic behavior of polymers under such conditions [182]. The second reason making this field intriguing for polymer science is the possibility to study chain dynamics under topological model constraints in the form of artificial tubes. In the following we will focus on this latter point. The tube introduced in the frame of the Doi/Edwards reptation model for the treatment of bulk systems of entangled polymers is a fictitious one. As outlined above, the laws predicted on this basis (see Table 1) can provide only a rather crude picture failing to account for numerous experimental findings quantitatively as well as qualitatively. It may therefore be helpful to study chain dynamics in tube-like pores of a physically real nature.

102

R. Kimmich · N. Fatkullin

The diffusion and relaxation behavior of diverse oligomers and polymers has been studied in nanoporous silica glasses [183]. Both measuring techniques provide clear evidence for modified chain dynamics compared with the bulk. However, the problem with this sort of system is that interactions of the polymers with the pore walls play an important role and must be distinguished from the geometrical confinement effect. A corresponding analysis was possible by comparison of polymer data with data obtained with short oligomers of the same chemical species. In contrast to the polymers, the oligomers were assumed to be subject to adsorption but not to modifications of the chain modes by geometrical confinement. Subtraction of the oligomer relaxation rates from those measured with polymers in the pores suggests a spin–lattice relaxation dispersion reduced for the influence of geometrical confinements on the chain-mode distribution. Actually a power law dispersion reproducing that predicted for limit (II)DE of the tube/reptation model (see Table 1) could be elucidated this way. A more direct verification of tube/reptation features was possible with systems where the solid matrix and the mobile polymer chains confined to nanopores are of similar organic chemical composition. In the experiments referred to in the following, linear polymers were confined in a solid, that is strongly cross-linked, polymer environment. Under such conditions, the geometry effect can be expected to dominate whereas the wall adsorption phenomenon is of negligible influence. This sort of system was prepared in the form of so-called semiinterpenetrating networks. Preparation details are described in Ref. [184]. The matrix

Fig. 43. Transmission electron micrograph of a replica of a freeze-fractured surface of polyethyleneoxide Mw=6,000 in PHEMA [11]. The pore channels have a width of about 10 nm

Polymer Chain Dynamics and NMR

103

consisted of cross-linked polyhydroxyethyl methacrylate (PHEMA). Linear polyethyleneoxide (PEO) was incorporated in the 10-nm pores. The molecular weights of the PEO samples used in experiment were chosen large enough to ensure that the root mean squared random-coil diameter in bulk exceeds the pore diameter. Figure 43 shows an electron micrograph of pore channels in this material having a width of about 10 nm. 5.1 Diffusion in Pores Segment diffusion in pores suggests itself as a typical model scenario representing the premisses of the tube/reptation model. NMR diffusometry is suitable to probe the time or length scales of the Doi/Edwards limits (II)DE, (III)DE and beyond. Since the wall adsorption effect in the PHEMA system is expected to be negligible, one can therefore expect that the reptation features of the anomalous segment diffusion regime, especially with respect to limit (III)DE, are faithfully rendered by the experiments. Figure 44 shows typical echo attenuation curves recorded with PEO in a solid PHEMA matrix [186]. The good coincidence of the theoretical curves calculated on the basis of Eqs. 76–79 for all accessible values of the experimental parameters k and t for different molecular weights [11] corroborates the validity of the tube/reptation model for linear polymers confined to arti-

Fig. 44. Echo attenuation curves for polyethyleneoxide, Mw=11,200, confined to PHEMA pores at 80 C as a function of the squared wave number, k2, for different diffusion times. The solid lines represent a fit of Eqs. 76–79 to the experimental data. The tube diameter is found to be a=(9€1) nm as the only fitting parameter. Other parameter values such as N=Mw/853, D0=9.661010 m2/s, and b=8.381010 m were taken from the literature [180, 187]

104

R. Kimmich · N. Fatkullin

ficial nanopores in a solid matrix. Very remarkably the tube diameter a (as the only free parameter) fitted to the diffusion data coincides with the pore diameter determined with other techniques such as electron microscopy, Xray scattering or NMR spin diffusion [184]. 5.2 Spin–Lattice Relaxation Dispersion in Pores Field-gradient NMR diffusometry experiments tend to be largely dominated by the time and length scales of limit (III)DE. On the other hand, the much shorter time scale of limit (II)DE can specifically be examined by NMR relaxometry, which under suitable conditions can indirectly probe translational diffusion of polymer segments. The laws predicted in Table 1 for anomalous segment diffusion on the one hand and spin–lattice relaxation on the other are based on the very same translational segment displacement mechanisms. They stipulate each other compellingly. Spin–lattice relaxation at low frequencies, as they can be covered with the aid of field-cycling NMR relaxometry, is therefore suitable to extend the range of field-gradient NMR diffusometry toward much shorter times. The total proton frequency range that can be probed by NMR spin–lattice relaxation techniques is 103 Hz < n < 109 Hz. For the present application, deuteron resonance selectively applied to perdeuterated polymers confined to the pores is superior to proton resonance which, unlike the situation in field-gradient experiments, is affected by signals from the matrix and flipflop spin diffusion across the matrix. The deuteron frequency range is shifted by a factor of 0.15 to lower frequencies. This frequency window largely matches the time scale of chain modes of polymers with medium molecular masses. The exceptional frequency and molecular weight dependence for the spin–lattice relaxation time expected for limit (II)DE, T1 / M0 w3=4 ðwts 1 wte Þ

ð187Þ

(see Table 1), is particularly indicative for reptational segment diffusion. Figure 45a shows the frequency dependence of the deuteron spin–lattice relaxation time of perdeuterated PEO of different molecular weights in a solid PHEMA matrix [95,185]. In the frequency regime, where the standard Bloch/Wangsness/Redfield relaxation theory is applicable, the law given in Eq. 187 is reproduced as T1 / Mw00:05 n0:750:02 :

ð188Þ

The experimental deuteron frequency range in which this frequency dependence was observed is 5105 Hz < n < 6107 Hz. De Gennes prediction for limit (II)DE has thus been verified for polymers confined in artificial

Polymer Chain Dynamics and NMR

105

Fig. 45a, b. Frequency dependence of the deuteron spin–lattice relaxation time of perdeuterated PEO confined in 10-nm pores of solid PHEMA at 80 C (a) and in bulk melts (b) [95, 185]. The dispersion of the confined polymers verifies the law T1 / Mw0 w0:75 at high frequencies as predicted for limit (II)DE of the tube/reptation model (see Table 1). The low-frequency plateau observed with the confined polymers indicates that the correlation function implies components decaying more slowly than the magnetization relaxation curves, so that the Bloch/Wangsness/Redfield relaxation theory [2] is no longer valid in this regime. The plateau value corresponds to the transverse relaxation time, T2, for deuterons extrapolated from the high-field value measured at 9.4 T

tubes in full accordance with the theory. This is in contrast to the bulk behavior of the very same polymers studied with deuteron resonance again. The data in Fig. 45b reproduce features observed with proton and deuteron resonance with bulk melts of other polymer species as discussed above (see Figs. 35 and 36). Polymer chains in bulk melts must obviously have additional degrees of freedom not existing under pore confinements. 5.3 Theoretical Crossover from Rouse to Reptation Dynamics The theoretical background of the confinement effect in (artificial) tubes was recently examined in detail with the aid of an analytical theory as well as with Monte Carlo simulations [70]. The analytical treatment referred to a polymer chain confined to a harmonic radial tube potential. The computer simulation mimicked the dynamics of a modified Stockmayer chain in a tube with “hard” pore walls. In both treatments, the characteristic laws of the tube/reptation model were reproduced. Moreover, the crossover from reptation (tube diameter equal to a few Kuhn segment lengths) to Rouse dy-

106

R. Kimmich · N. Fatkullin

Fig. 46. Theoretical mean squared segment displacement of a chain confined in a randomly coiled tube versus time according to the harmonic radial potential theory [70]. The tube diameter d is given in multiples of the Kuhn segment length b. The crossover tendency to free, unconfined Rouse chain dynamics with increasing tube diameter is obvious. The mean squared displacement is given in units b2, the diffusion time t in units of the segmental fluctuation time ts. The chain length was assumed to be N=1,600 Kuhn segments. The three “anomalous” Doi/Edwards limits (see Table 1) are reproduced with finite tube diameters

namics (tube diameter “infinite”) was demonstrated by varying the tube diameter. Figure 46 shows the time dependence of the mean squared segment displacement as predicted by the harmonic radial potential theory [70]. The three anomalous diffusion limits, (I)DE, (II)DE, and (III)DE, of the tube/reptation model are well reproduced. Note the extended width of the transition regimes between these limits, which should be kept in mind when discussing experimental data with respect to a crossover between different dynamic limits. Increasing the effective tube diameter is accompanied by the gradual transition to Rouse-like dynamics of an unconfined chain (where entanglement effects are not considered). The spin–lattice relaxation dispersion was derived with the same sort of theory. Figure 47 shows data obtained under the same conditions as assumed for the mean squared displacement data in Fig. 46. Again the dispersion most specific for the tube/reptation model, namely T1/w0.75 which is predicted for limit (II)DE, was perfectly reproduced at low frequencies.

Polymer Chain Dynamics and NMR

107

Fig. 47. Spin–lattice relaxation dispersion for a chain of N=1,600 Kuhn segments (of length b) confined to a randomly coiled tube with a harmonic radial potential with varying effective diameters d˙. The data were calculated with the aid of the harmonic radial potential theory [70]. ~c is a constant. At low frequencies the curves visualize the crossover from Rouse dynamics depending on the effective tube diameter. The latter case is described by a T1 dispersion proportional to w3/4 characteristic for limit (II)DE of the tube/ reptation model

6 Concluding Remarks NMR may be considered as a particularly versatile class of investigation methods suitable for polymer dynamics studies. In particular, field-cycling NMR relaxometry employed in parallel with field-gradient NMR diffusometry is an unmatched combination of methods for the elucidation of features of chain dynamics. A great wealth of clearly documented phenomena for different measurands, experimental parameters, and different polymer species in different environments and under different thermodynamic conditions were discovered, and appear to be suitable for direct comparisons with theoretical model predictions. One can say that the experimental data available so far already render a closed picture from the empirical point of view. Transverse and longitudinal NMR relaxometry of 1H and 13C nuclei was shown to be governed by three components of chain dynamics. With respect to tests of theoretical model concepts, the most important one is component B which reflects the influence of chain modes and can be probed with the field-cycling technique. Field-gradient NMR diffusometry is suitable for recording translational displacement properties by self-diffusion. This in particular refers to the anomalous segment displacement regime. Center-of-mass diffusion is also accessible this way but must be handled with some care because of the experimental limitation of the maximum diffusion time. Furthermore the in-

108

R. Kimmich · N. Fatkullin

fluence of flip-flop spin diffusion must be taken into account when examining long polymers. Three basic model theories have been considered: the Rouse model, the tube/reptation concept, and the renormalized Rouse formalism. Depending on the sample system and the experimental conduct, characteristic features of all these theories have been shown. Some spectacular predictions of theories were verified, others were ruled out. The frequency dependence of the spin–lattice relaxation time predicted by the Rouse model was verified with polymer melts for Mw<Mc in accordance with the segmental fluctuation time determined from the T1 minimum condition. Melts with Mw>>Mc did not show any such behavior in the shorttime limit although predicted so by all three model theories. On the other hand, dilution of the polymer by a low-molecular solvent increases Mc and diminishes the entanglement effect. Under such conditions, Rouse-like behavior was observed. The tube/reptation model of entangled polymer dynamics suggests a number of peculiar anomalous-diffusion limits that were consistently and quantitatively verified in artificial tubes of a solid porous matrix with the aid of field-cycling NMR relaxometry and field-gradient NMR diffusometry. This clear corroboration of a model prediction is however in contrast to the dynamics concluded for bulk melts. In that case neither the prediected T1 dispersion nor the anomalous segment diffusion behavior was found with respect to the frequency and molecular weight dependences. The assumption of static fictitious tubes as a replacement scheme for the entangling matrix effect is obviously too crude for bulk melts, and does not render the features of polymer dynamics correctly. Based on the generalized Langevin equation, the renormalized Rouse models suggest dynamic high- and low-mode-number limits as an implicit structural feature of this equation of motion. This is a stand-alone prediction of paramount importance independent of any absolute values of power law exponents that arise and are measured in the formalism and in experiment, respectively. The two limits manifesting themselves as power law spin–lattice relaxation dispersions were clearly identified in bulk melts of entangled polymers of diverse chemical species. Apart from these two relaxation dispersion regimes, which are mainly based on intrasegment spin interactions (and possibly nearest neighbor intersegment contributions), a third dispersion region specific for dipolarcoupled nuclei exists at low frequencies. This was shown to be due to (longdistance) dipolar interactions being relevant for protons but not for deuterons. A most important finding in general and for establishing of model theories is the fact that segment dynamics is affected by microstructural details already at relatively short times. The local fluctuations of a Kuhn segment typically occur on a time scale shorter than 1010 s and on a length scale of

Polymer Chain Dynamics and NMR

109

up to 1 nm. It was shown that factors such as chain entanglements, crosslinking or mesomorphic order quite amazingly, and contrary to most model expectations, have an influence on segment dynamics already rather close to these time and length scales. This finding became evident from the relaxometry studies reported and was also observed in the literature [129]. On the other hand, chain modes with low mode numbers and even global, molecular weight dependent motions corresponding to chain relaxation times beyond the Rouse relaxation time do show up at the predicted time and length scales. Acknowledgments We thank Elmar Fischer, Alexei Denissov, Margarita Kroutieva, Hans Wiringer, and Birgit K rner for discussions and excellent assistance in the preparation phase of this article. Grants by the DFG, the Volkswagen-Stiftung, CRDF, and RFBR are gratefully acknowledged.

References 1. Doi M, Edwards SF (1986) The theory of polymer dynamics. Clarendon, Oxford 2. Kimmich R (1997) NMR tomography, diffusometry, relaxometry. Springer, Berlin Heidelberg New York 3. Fatkullin N, Kimmich R (1995) Phys Rev E 52:3273 4. Torrey HC (1956) Phys Rev 104:563 5. Stejskal EO, Tanner JE (1965) J Chem Phys 42:288 6. Tanner JE, Stejskal EO (1968) J Chem Phys 49:1768 7. Saarinen TR, Johnson CS (1988) J Magn Reson 78:257 8. Kimmich R, Unrath W, Schnur G, Rommel E (1991) J Magn Reson 91:136 9. Fischer E, Kimmich R, Fatkullin N (1996) J Chem Phys 104:9174 10. Fischer E, Kimmich R, Fatkullin N (1997) J Chem Phys 106:9883 11. Fischer E, Kimmich R, Beginn U, M ller M, Fatkullin N (1999) Phys Rev E 59:4079 12. Fischer E, Kimmich R, Fatkullin N, Yatsenko G (2000) Phys Rev E 62:775 13. Fujara F, Geil B, Sillescu H, Fleischer G (1992) Z Phys B 88:195 14. Kimmich R, Fischer E (1994) J Magn Reson A 106:229 15. Kimmich R, Fischer E, Callaghan P, Fatkullin N (1995) J Magn Reson A 117:53 16. Grinberg F, Kimmich R (1995) J Chem Phys 103:365 17. Abragam A (1961) The principles of nuclear magnetism. Clarendon, Oxford 18. Kimmich R (1980) Bull Magn Reson 1:195 19. Noack F (1986) Progr NMR Spectr 18:171 20. Kimmich R (1996) Molecular motions: T1 frequency dispersion in biological systems. In: Grant DM, Harris RK (eds) Encyclopedia of nuclear magnetic resonance, vol 5. Wiley, Chichester, pp 3083–3088 21. Seitter R, Kimmich R (1999) Magnetic resonance: relaxometers. In: Lindon J, Trantar G, Holmes J (eds) Encyclopedia of spectroscopy and spectrometry. Academic, London, pp 2000–2008 22. Anoardo E, Grinberg F, Vilfan M, Kimmich R (2004) Chem Phys 297:99 23. Cohen-Addad JP (1993) Progr NMR Spectr 25:1 24. Guillermo A, Cohen-Addad JP, Bytchenkoff D (2000) Chem Phys 113:5098 25. Cohen-Addad JP, Guillermo A (2000) Phys Rev Lett 85:3432

110

R. Kimmich · N. Fatkullin

26. Brereton MG (1990) Macromolecules 23:1119 27. Ball RC, Callaghan PT, Samulski ET (1997) J Chem Phys 106:7352 28. Callaghan PT, Samulski ET (1998) Macromolecules 31:3693 29. Fischer E, Grinberg F, Kimmich R, Hafner S (1998) J Chem Phys 109:846 30. Maxwell RS, Balazs B (2002) J Chem Phys 116:10492 31. Graf R, Heuer A, Spiess HW (1998) Phys Rev Lett 80:5738 32. Dollase T, Graf R, Heuer A, Spiess HW (2001) Macromolecules 34:298 33. Schnur G, Kimmich R (1988) Chem Phys Lett 144:333 34. K pf M, Schnur G, Kimmich R (1988) J Polym Sci Polym Lett 26:319 35. Kimmich R, Schnur G, K pf M (1988) Progr NMR Spectr 20:385 36. Kimmich R, K pf M, Callaghan P (1991) J Polym Sci Polym Phys 29:1025 37. Volkenstein MV (1963) Configurational statistics of polymer chains. Interscience, New York 38. Birshtein TM, Pticin OB (1966) Conformation of macromolecules. Interscience, New York 39. Flory PG (1969) Statistical mechanics of chain molecules. Interscience, New York 40. Yamakava H (1971) Modern theory of polymer solutions. Harper and Row, New York 41. de Gennes PG (1979) Scaling concepts in polymer physics. Cornell University Press, Ithaka 42. Grosberg AYu, Khokhlov AR (1994) Statistical physics of macromolecules. AIP, New York 43. Gotlib YuYa, Darinskii AA, Svetlov YuE (1986) Physical kinetics of macromolecules. Khimia, Leningrad (in Russian) 44. Grosberg AYu, Khokhlov AR (1997) Giant molecules: here, there, and everywhere... Academic, San Diego 45. Kargin VA and Slonimskii GL (1949) Journal Fizhimii (USSR) 23:563 46. Rouse PJ (1953) J Chem Phys 21:1272 47. Fatkullin N, Kimmich R, Weber HW (1993) Phys Rev E 47:4600 48. Kimmich R, Fatkullin N, Weber HW, Stapf S (1994) J Non-Cryst Solids 172–174: 689 49. Fatkullin N, Kimmich R (1994) J Chem Phys 101:822 50. Khazanovich TN (1963) Polymer Sci USSR 4:727 51. Ullman R (1965) J Chem Phys 43:3161 52. Ferry JD (1980) Viscoelastic properties of polymers. Wiley, New York 53. Edwards SF (1967) Proc Phys Soc 92:9 54. de Gennes PG (1971) J Chem Phys 55: 572 55. Doi M, Edwards SF (1978) J Chem Soc Faraday Trans II 74:1789 56. Klein J (1978) Macromolecules 11:852 57. Doi MJ (1983) Poly Sci Poly Phys 21:667 58. Guenza M (2002) Phys Rev Lett 88:025901 59. Rubinstein M (1987) Phys Rev Lett 59:1946 60. de Cloizeaux (1988) J Europhys Lett 5:437 61. Graessley WW (1982) Adv Polym Sci 47:1 62. Pearson D (1987) Rubber Chem Tech 60:437 63. Marruci G (1985) J Polym Sci Polym Phys 23:159 64. Watanabe H, Tirrel M (1989) Macromolecules 22:927 65. Doi M, Pearson D, Kornfield J, Fuller G (1989) Macromolecules 22:1488 66. Fixman M (1991) J Chem Phys 95:1410 67. Gao J, Weiner JH (1992) Macromolecules 25:1348 68. Gao J, Weiner JH (1994) Science 266:748 69. Loriot G, Weiner JH (1998) J Polym Sci Polym Phys 36:143

Polymer Chain Dynamics and NMR

111

70. Denissov A, Kroutieva M, Fatkullin N, Kimmich R (2002) J Chem Phys 116:5217 71. Kimmich R (1975) Polymer 16:851 72. Kimmich R (2002) Chem Phys 284:253 73. Ardelean I, Kimmich R (2003) Ann Rep NMR Spectr 49:43 74. Fatkullin N, Kimmich R (1999) JETP Lett 69:762 75. Fatkullin N, Kimmich R (1999) Macromol Symp 146:103 76. Padding JT, Briels WJ (2001) J Chem Phys 115:2446 77. Fatkullin N (2002) J Non-Cryst Solids 307–310:824 78. Skolnick J, Kolinski A (1990) Adv Chem Phys 78:223 79. Kremer K, Grest GS (1990) J Chem Phys 92:5057 80. Kremer K, Grest GS (1992) J Chem Soc Faraday Trans 88:1707 81. Pakula T (1996) Recent Res Devel Polym Sci 1:101 82. Binder K, Paul W (1997) J Polym Sci Polym Phys 35:1 83. Pakula T (1998) Computational Theor Polym Sci 8:21 84. Shaffer JS (1995) J Chem Phys 103:761 85. Binder K, Paul W (1997) J Polym Sci Polym Phys 35:1 86. Khalatur PG (1996) Computer simulations in polymer systems. In: Kuchanov SI (ed) Mathematical methods in contemporary chemistry. Gordon and Breach, New York 87. Padding JT, Briels WJ (2002) J Chem Phys 117:925 88. Paul W (2002) Chem Phys 284:59 89. Hermann MF (1990) J Chem Phys 92:2043 90. Hermann MF, Panajotova B, Lorenz KT (1996) J Chem Phys 105:1153 91. Douglas JF, Hubbard JB (1991) Macromolecules 24:3163 92. Chatterjee AP, Loring RF (1995) J Chem Phys 103:4711 93. Ngai KL, Phillies GDJ (1996) J Chem Phys 105:8385 94. Ngai KL (1999) Macromol Symp 146:117 95. Kimmich R, Seitter R-O, Beginn U, M ller M, Fatkullin N (1999) Chem Phys Letters 307:147 96. Zwanzig R (1974) J Chem Phys 60:2717 97. Bixon M, Zwanzig R (1978) J Chem Phys 68:1890 98. Schweizer KS (1989) J Chem Phys 91:5802 99. Schweizer KS (1989) J Chem Phys 91:5822 100. Schweizer KS (1993) Physica Scripta T49:99 101. Fuchs M, Schweizer KS (1997) J Chem Phys 106:347 102. Guenza M, Schweizer KS (1997) J Chem Phys 106:7391 103. Schweizer KS, Fuchs M, Szamel G et al. (1997) Macromol Theory Simul 6:1037 104. Guenza M (1999) J Chem Phys 110:7574 105. Fatkullin N, Kimmich R, Kroutieva M (2000) JETP 91:150 106. Genz U (1994) Macromolecules 27:3501 107. Genz U, Vilgis TA (1994) J Chem Phys 101:7101 108. Genz U, Vilgis TA (1994) J Chem Phys 101:7111 109. Zwanzig R (1960) J Chem Phys 33:1336 110. Zwanzig R (1961) Phys Rev 124:985 111. Mori H (1965) Progr Theor Phys 33:423 112. Mori H (1965) Progr Theor Phys 34:765 113. Hansen JP, McDonald (1991) Theory of simple liquids, 2nd edn. Academic, London 114. Baluccani U, Zoppi M (1994) Dynamics of the liquid state. Clarendon, Oxford 115. Berne BJ, Pecora R (1976) In: Berne BJ (ed) Dynamical light scattering. Wiley, New York 116. Edwards SF, Grant JW (1973) J Phys A Math Nucl Gen 6:1169

112

R. Kimmich · N. Fatkullin

117. Edwards SF, Grant JW (1973) J Phys A Math Nucl Gen 6:1189 118. Ronca G (1983) J Chem Phys 79:1031 119. Fixman MF (1988) J Chem Phys 89:3892 120. Hess W (1988) Macromolecules 21:2620 121. Rostiashvili VG (1990) Sov Phys JETP 70:563 122. Pokrovskii VN (1992) Sov Phys Usp 35:384 123. Kimmich R, Bachus R (1982) Coll Polym Sci 260:911 124. Kimmich R, K pf M (1989) Progr Coll Polym Sci 80:8 125. Weber HW, Kimmich R (1993) Macromolecules 26:2597 126. Gotlib YY, Torchinskii IA, Shevelev VA (2001) Polym Sci A 43:1066 127. Gotlib YY, Torchinskii IA, Shevelev VA (2002) Polym Sci A 44:206 128. Voigt G, Kimmich R (1980) Polymer 21:1001 129. Qui XH, Ediger MD (2002) Macromolecules 35:1691 130. Allen G, Connor TM, Pursey H (1963) Trans Faraday Soc 59:1525 131. Kimmich R, Gille K, Fatkullin N, Seitter R, Hafner S, M ller M (1997) J Chem Phys 107:5973 132. Koch H, Bachus R, Kimmich R (1980) Polymer 21:1009 133. Schneider H, Hiller W (1990) J Polym Sci Polym Phys 28:1001 134. Singer A, Hiller W (1985) Polym Bull 14:469 135. Manelis GB, Erofeev LN, Provotorov BN, Khitrin AK (1989) Sov Sci Rev B Chem 14:1 136. Kuhn W, Barth P, Hafner S, Simon G, Schneider H (1994) Macromolecules 27:5773 137. Cohen-Addad JP, Guillermo A (1984) J Polym Sci Polym Phys 22:931 138. Kimmich R (1984) Polymer 25:187 139. Kimmich R, Rosskopf E, Schnur G, Spohn KH (1985) Macromolecules 18:810 140. Weber HW, Kimmich R, K pf M, Ramik T, Oeser R (1992) Progr Coll Polym Sci 90:104 141. K pf M, Schnur G, Kimmich R (1988) Macromolecules 21:3340 142. Doi M (1981) J Polym Sci Polym Lett 19:165 143. K pf M (1991) PhD thesis, Universitt Ulm 144. Kimmich R (1985) Helv Phys Acta 58:102 145. Doolittle AK (1951) J Appl Phys 22:1471 146. Fox TG, Gratch S, Lashaek S (1956) In: Eirich FR (ed) Rheology, vol.1. Academic, New York, p 431 147. Bailey RT, North AM, Pethrick RA (1981) Molecular motion in high polymers. Clarendon, Oxford 148. Fleischer G (1984) Polym Bull 11:75 149. Fleischer G (1987) Coll Polym Sci 265:89 150. von Meerwall E, Ferguson RD (1982) J Polym Sci Polym Phys 20:1037 151. Kimmich R, Peters A, Spohn K-H (1981) J Membrane Sci 9:313 152. Bachus R and Kimmich R (1983) Polym Communications 24:317 153. Kimmich R, Weber HW (1993) J Chem Phys 98:5847 154. Kimmich R, Fatkullin N, Seitter R-O, Gille K (1998) J Chem Phys 108:2173 155. Kimmich R, Stapf S, M ller M, Out R, Seitter R-O (1994) Macromolecules 27:1505 156. Link T, Kimmich R (2000) unpublished 157. Fenchenko KV (1997) Polym Sci B 39:146 158. Herman, MF (2000) J Chem Phys 112:3040 159. Godovsky YK, Papkov VS (1989) Adv Polym Sci 88:129 160. K gler G, Loufakis K, M ller M (1990) Polymer 31:1538 161. Pincus P (1969) Solid State Commun 7:415 162. Blinc R, Hogenboom D, OReilly D, Peterson E (1969) Phys Rev Lett 23:969

Polymer Chain Dynamics and NMR

113

163. Doane JW, Johnson DL (1970) Chem Phys Lett 6:291 164. Ukleja P, Pirs J, Doane JW (1976) Phys Rev A 14:414 165. Dong RY (1983) Isr J Chem 23:370 166. Vilfan M, Kogoj M, Blinc R (1987) J Chem Phys 86:1055 167. Zeuner U, Dippel T, Noack F, M ller K, Mayer C, Heaton N, Kothe G (1992) J Chem Phys 97:3794 168. Grinberg F, Kimmich R, M ller M, Molenberg A (1996) J Chem Phys 105:9657 169. Bachus R, Kimmich R (1983) Polymer 24:964 170. Maklakov AI, Skirda VD, Fatkullin NF (1990) Self diffusion in polymer melts and solutions. In: Cheremisinoff NP (ed) Encyclopedia of fluid mechanics, vol 9: polymer flow engineering. Gulf, Houston 171. Manz B, Callaghan PT (1997) Macromolecules 30:3309 172. Komlosh ME, Callaghan PT (1998) J Chem Phys 102:1648 173. Tao H, Lodge TP, von Meerwall ED (2000) Macromolecules 33:1747 174. Lodge TP (1999) Phys Rev Letters 83:3218 175. Fleischer G (1985) Polymer 26:1677 176. Grinberg F, Garbarczyk M, Kuhn W (1999) J Chem Phys 111:11222 177. Garbarczyk M, Grinberg F, Nestle N, Kuhn W (2001) J Polym Sci Polym Phys 39:2207 178. Rommel E, Kimmich R, Sp lbeck M, Fatkullin NF (1993) Progr Colloid Polym Sci 93:155 179. Kugler J, Fischer EW (1983) Makromol Chemie 184:2325 180. Smith GD, Yoon DY, Jaffe RL, Colby RH, Krishnamoorti R, Fetters LJ (1996) Macromolecules 29:3462 181. Fatkullin NF, Yatsenko GA, Kimmich R, Fischer E (1998) J Exp Theor Phys 87:294 182. de Gennes PG (1999) Advan Polym Sci 138:91 183. Stapf S, Kimmich R (1995) Macromolecules 29:1638 184. Beginn U, Fischer E, Pieper T, Mellinger F, Kimmich R, M ller M (2000) J Polym Sci Polym Chem 38:2041 (note that a misprint occurred in that paper with the length scale specified in the electron micrograph given at Fig. 8) 185. Kimmich R, Fatkullin N, Seitter R-O, Fischer E, Beginn U, M ller M (1999) Macromol Symp 146:109 186. Fischer E, Beginn U, Fatkullin N, Kimmich R (2004) Macromolecules 37:3277 187. Graessley WW, Edwards SF (1981) Polymer 22:1329 Editor: Sam Edwards

Received: February 2003

APS (2004) 170:115--113 DOI 10.1007/b95533 Springer-Verlag 2004

Emerging Technologies for the 3D Analysis of Polymer Structures Hiroshi Jinnai1 · Yukihiro Nishikawa1 · Takayuki Ikehara2 · Toshio Nishi3 (*) 1

Department of Polymer Science and Engineering, Kyoto Institute of Technology, 606-8585 Kyoto, Japan [email protected] 2 Department of Applied Chemistry, Faculty of Engineering, Kanagawa University, 3-27-1 Rokkakubashi, Kanagawa-ku, 221-8686 Yokohama, Japan 3 Department of Organic and Polymeric Materials, School of Science and Engineering, Tokyo Institute of Technology, 2-12-1 Ohokayama, Meguro-ku, 152-8551 Tokyo, Japan

1

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

118

2 2.1 2.2

3D Microscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Laser Scanning Confocal Microscopy (LSCM) . . . . . . . . . . . . . . . . . . Transmission Electron Microtomography (TEMT) . . . . . . . . . . . . . . .

120 121 123

3 3.1 3.2 3.2.1 3.2.2 3.2.3 3.3

Digital Image Analysis of 3D Structures. 3D Reconstruction . . . . . . . . . . . . . Curvature Distribution Measurements . . Surface Curvatures . . . . . . . . . . . . . Parallel Surface Method (PSM) . . . . . . Sectioning and Fitting Method (SFM) . . Surface Topology . . . . . . . . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

125 125 126 127 128 129 132

. . . . . .

136 136 137 139 139 141

. . .

144 146 147

. . . . . . . . . .

152 152

. . . . .

154

. . . . .

155

. . . . .

157

4

Time Evolution of Bicontinuous Structure in Spinodal Interface of a Binary Polymer Mixture . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Basics of Phase Separation in Binary Polymer Mixutures . . . . . . . . . . 4.2 Direct 3D Visualization of Phase-Separating Bicontinuous Structures. . . . 4.3 3D Structural Analysis of Phase-Separating Bicontinuous Structures . . . . 4.3.1 Scaled Structure Factor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.2 Interfacial Curvature Measurement: Comparison Between LSCM and TRLS 4.3.3 Curvature Distribution Measurements of Phase-Separating Bicontinuous Structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4 Scaling Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5 Effects of Surface Wetting and Confinement on Spinodal Decomposition . 5

Direct Measurement of Interfacial Curvature Distributions in a Bicontinuous Block Copolymer Nanostructure . . . . . . . . . 5.1 Basics of Microphase-Separated Morphologies in Block Copolymers 5.2 Direct 3D Visualization and Curvature Distribution of Bicontinuous Block Copolymer Nanostructure . . . . . . . . . . . 5.3 Geometrical and Topological Analysis of Bicontinuous Block Copolymer Nanostructure . . . . . . . . . . . 5.3.1 Comparison Between Experiment and Theory in Terms of Interfacial Curvature Distribution . . . . . . . . . . . . . . . . . .

116 6

H. Jinnai et al. Geometrical Similarity/Difference Between Polymer Blend and Block Copolymer Structures. . . . . . . . . . . . . . . . . . . . . . . . .

158

Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

163

References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

164

7

This review covers recent progress of studies using new methods for analyzing polymer structures, with emphasis on three-dimensional (3D) microscopy, e.g., laser scanning confocal microscopy (LSCM) and transmission electron microtomography (TEMT). These methods have been applied to morphological studies of structures in polymer alloys over the past few years. We review some of the studies dealing with 3D structures of binary polymer blends and block copolymers that are self-assembled during the phase separation processes and/or phase transition. Typical sizes of such self-assembled structures are of the order of micro- and nanometers, respectively. A great deal of new structural information, which has never been obtained from conventional microscopy or various scattering methods, can be evaluated directly from the 3D volume data. The structural information obtained from 3D microscopy offers essential insight into the physics of nonlinear, nonequilibrium phenomena and the statistical mechanics of long-chain molecules. Keywords Polymer alloy · 3D microscopy · 3D digital image analysis · Bicontinuous structures Abbreviations and Symbols Area of i-th triangles (generated by MCA) sharing the j-th POI Atri(i;j) CMC Constant mean curvature CT Computerized tomography d Signed displacement of the parallel surface D Thickness of (blend) specimen Diameter (size) of an object reconstructed in CT DCT DPB Deuterated polybutadiene f Copolymer composition Styrene volume fraction in microphase-separated structure fS of SIS block copolymer E Number of edges of faces subdividing the surface F Number of faces subdividing the surface F(x) Scaled structure factor f(x,y) Intersection of an object H Mean curvature ~ H Scaled mean curvature hHi Area-averaged mean curvature I(q,t) Scattering intensity in TRLS experiment I(x,y,z) Intensity of fluorescence from a particular point in a focal plane (x–y plane) at a depth z K Gaussian curvature ~ K Scaled Gaussian curvature hKi Area-averaged Gaussian curvature L Crystallographic unit cell edge LS Light scattering

Emerging Technologies for the 3D Analysis of Polymer Structures LSCM MCA N NCT Nj NA Ntri n ntri p PB p(r,j) P(H,K) PH(H) ~H H; ~ t P pi PK(K) ~ t ~K K; P POI PSM q qm(t) qc r RI Rm Rm,LS Rm,LSCM Rg S SCFT SD SFM Si SIS S(q) t TDGL TEM TEMT u and v V Vs z c dA(j)

117

Laser scanning confocal microscopy Marching cubes algorithm Number of pixels along the edge of the image Number of projections in CT Coordination number at a junction Numerical aperture of an objective Total number of triangles comprising interface generated by MCA Normal vectors at vertices of the polygon generated by MCA Normal vector of each triangle generated by MCA Positional vector of a surface Polybutadiene Projection at an angle j Joint probability density of surface curvatures Marginal probability densities of the mean curvature Scaled marginal probability densities of the mean curvature Coordinates of the i-th vertices of the triangle generated by MCA Marginal probability density of the Gaussian curvature Scaled marginal probability density of the Gaussian curvature Point of interest at a surface Parallel surface method Wave number Wave number at which I(q,t) shows a maximum Crossover wave number from q6 to q4 with increasing q in I(q,t) of spinodally decomposing polymer mixtures Resolution of reconstructed image in CT Roughness index Area-averaged mean radius in Tomitas scattering theory Mean radius estimated from LS based on Tomitas scattering theory (Eqs. 28 and 29) Mean radius estimated from LSCM based on Tomitas scattering theory (Eq. 29) Radius of gyration of polymers (Total) interfacial area Self-consistent field theory Spinodal decomposition Sectioning and fitting method Area of i-th neighboring triangles generated by MCA Poly(styrene-b-isoprene-b-styrene) triblock copolymer Scattering structure factor Phase-separation time Time-dependent Ginzburg–Landau equation Transmission electron microscopy Transmission electron microtomography Curvilinear coordinates of a surface Number of vertices of faces subdividing the surface Volume of the whole system Depth along the optical axis of LSCM Euler–Poincar characteristic Local area assigned to j-th POI

118 DF DH DK DZ hh(t)2i q ki l lLS Lm(t) sH P (t) f fPB j

H. Jinnai et al. Full width at half maximum (fwhm) of optical sections in LSCM observations Class interval of H Class interval of K Increment along depth direction of LSCM Mean squared refractive index fluctuations Scattering angle in TRLS experiments Principal curvatures (i=1 and 2) Wavelength of laser of LSCM Wavelength of laser in TRLS experiments Length characterizing the global size of SD bicontinuous structures Standard deviation of the mean curvature distribution Surface area per unit volume Volume fraction of one of the phases in polymer mixture Volume fraction of the PB-rich phase in DPB/PB mixture Angle of the projection slice in computerized tomography (CT)

1 Introduction Polymer materials are ubiquitous in our daily life. Such materials often consist of more than one species of polymer and thus become multicomponent systems, such as polymer blends [1,2] and block copolymers [3]. Due to repulsive interaction between the constituent polymers, the multicomponent polymer materials involve “phase separation”. Studies to characterize the phase-separated structures inside the materials have been growing intensively over the past three decades. Academic interest in the complex fluids (to which polymeric systems belong) as well as ceaseless industrial need for developing new materials activated such studies. In academia, for example, pattern formation and self-assembling processes of binary polymer blends are one of the most fascinating research themes in nonlinear, nonequilibrium phenomena. Block copolymers likewise self-organize into (equilibrium) phase-separated nanostructures (termed “microphase-separated structures” in contrast to the “macrophaseseparated structures” in the polymer blend). Since it is required for the block copolymers to place their junctions at the interface and thus the microdomain-forming blocks must uniformly fill space in the most entropically favored manner, the block copolymer morphologies are often highly organized. Studies of the block copolymer morphologies belong to the statistical mechanics of long-chain molecules. In industry, such phase-separated polymer systems have been found important to achieve superior physical properties. Hence, the structure–property relationship in multicomponent polymeric materials is of significant importance, basic studies on which eventually render new designs of polymer materials satisfying the diverse requirements of industry.

Emerging Technologies for the 3D Analysis of Polymer Structures

119

Up to now, morphological studies of the multicomponent polymeric materials have been carried out by various microscopic and scattering methods. Optical microscopes, transmission electron microscopes (TEM), scanning electron microscopes (SEM), and atomic force microscopes (AFM) are commercially available and widely used. The biggest advantage to using such microscopes is that they offer intuitive real-space representation of morphologies by showing images. However, when it comes to “measurements”, especially in a quantitative way, the microscopes sometimes give only limited pieces of structural information with inferior statistical accuracy compared with scattering methods. The scattering techniques give statistically averaged structural information over the scattering volume, which is normally a lot bigger than the area of the microscopes. Although accurate, the scattering methods do not directly provide intuitive insight into the morphologies. Moreover, in general, the scattering methods may require knowledge of the morphologies beforehand to obtain structural parameters. In other words, for the complete characterization of the morphologies, one may need to know them first by the microscope and subsequently evaluate statistically the structural parameters by the scattering on the basis of the morphologies. Thus, the two methods have the pros and cons and are complementary to each other. According to the size of the morphologies, one may use an optical microscope together with light scattering (LS) for micron-scale morphologies and TEM (or SEM, AFM) with small-angle neutron (or X-ray) scattering for nanometer-scale structures. One of the biggest problems one might encounter in the course of the above conventional protocol is that the identification of complex structures by the microscopes is often inconclusive and hence interpretation of the scattering data would not be straightforward. The microscopes used so far are able to take two-dimensional (2D) (transmitted or surface) images of three-dimensional (3D) objects. The more complicated the morphologies are, the less convincing the interpretation of the 2D images usually become. It is thus requisite to develop microscopes that are capable of obtaining 3D images. Hereafter, we call such microscopes 3D microscopes and the methodology 3D-scopy or 3D microscopy. Due to these backgrounds, a couple of different types of 3D microscopes have been developed as described in Sect. 2. We emphasize that 3D microscopy should be accompanied by digital image analysis (see Sect. 3) that extracts useful and new structural information from the 3D volume data. In the present review, we will try to demonstrate that 3D microscopy has great advantages over the conventional methods to observe and analyze complex polymer structures. This review paper is organized in the following way. In Sect. 2, we briefly describe the basic principles of 3D microscopy that will be used later in this review paper. In Sect. 3, quantitative 3D image analysis for the 3D volume data on the basis of the geometry will be introduced. Section 4 is dedicated to the visualization of one of the transient

120

H. Jinnai et al.

structures observed in the polymer blend during the phase separation called spinodal decomposition (SD). It was found that the two domains form networks that coexist in 3D space (bicontinuous sructure). The stability of the interface between the two domains, the effects of preferential wetting and confinement on the SD process were examined using the (differential) geometry. 3D direct observation of the nanoscale structure of block copolymers will be discussed in terms of their stability in Sect. 5. The block copolymer morphology we dealt with exhibited bicontinuity similar to that of the one studied in the polymer blend. The effect of incorporation of the covalent bond (to form block copolymers) on the shape and regularity of the resulting morphologies is of particular interest, which will be discussed in Sect. 6. Finally, concluding remarks are given in Sect. 7.

2 3D Microscopy Figure 1 shows the spatial resolution of various types of microscopes and scattering methods. The figure includes 3D microscopy such as laser scanning confocal microscopy (LSCM), X-ray computerized tomography (X-ray CT), and transmission electron microtomography (TEMT). Although no experimental results obtained from the X-ray CT will be presented in the present review paper, we note that the microscopy [4] is particularly useful to

Fig. 1 Schematic illustration showing resolution of both microscopic and scattering methods. Abbreviations are the following: OM (optical microscopy), LSCM (laser scanning confocal microscopy), X-ray CT (X-ray computerized tomography), SEM (scanning electron microscopy), TEMT (transmission electron microtomography), ATF (atomic force microscopy), WAXS (wide-angle X-ray scattering), SAXS (small-angle X-ray scattering), LS (light scattering), USAXS (ultra-small-angle X-ray scattering), SANS (small-angle neutron scattering), and USANS (ultra-small-angle neutron scattering)

Emerging Technologies for the 3D Analysis of Polymer Structures

121

observe internal structures of opaque specimens. In the early 1990s, the spatial resolution of the X-ray CT was limited to ca. 100 m. Recently, a resolution comparable with that of the optical microscope (~1 m) has been achieved. It should be emphasized that, combining LSCM, X-ray CT, and TEMT, it is possible to establish a 3D microscopy whose resolution is over the wide range from nano- to micrometers. In what follows, we will briefly describe the principles and some applications for LSCM and TEMT. 2.1 Laser Scanning Confocal Microscopy (LSCM) After LSCM became commercially available in the late 1980s, the instrument generated an excitement among biologists. With LSCM, one can slice incredibly clean thin optical sections out of thick specimens, gain impressive 3D views at high resolution [5, 6]. The focal depth of the conventional optical microscopes is usually deep in comparison to its lateral resolution. This leads to the superposition of the out-of-focus images, and hinders the 3D interpretation of the images. Confocal microscopy has overcome this disadvantage by introducing a pinhole just in front of the detector as shown in Fig. 2. The solid line shows the opti-

Fig. 2 Optics of confocal microscopy. The incident light emitted from laser (1) is reflected by a dichroic mirror (2). The reflected light is focused on the specimen (4) through objective lens (3). At the focus the light may be reflected by the interior structure or the incident laser excites fluorescent molecules attached to the particular site (position) of the specimen. The reflected light or fluorescence from the focal plane refocuses at the confocal pinhole (5) and thus it passes the pinhole to reach detector (6). The out-of-focus light (fluorescence) is blocked by the confocal pinhole as shown by the dashed line

122

H. Jinnai et al.

cal path of reflected (or fluorescent) light in the focal plane of the objective lens. The reflected (or fluorescent) light focuses at the pinhole and reaches the detector. Simultaneously, the object may reflect the out-of-focus light (or emit the out-of-focus fluorescence), as shown by the dashed line in Fig. 2. In this case, simple ray tracing shows that the light (or fluorescence) reflected back to the confocal pinhole arrives as a defocused blur, only the central portion of which is detected and contributes to the image. In this way the system eliminates the images which do not lie within the focal region of the lens. The excellent depth resolution thus achieved, which is the full width at half maximum (fwhm) of optical sections, DF, is typically 1 m or may be less, depending on the optical setup. DF is a complicated function of an incident laser beam of wavelength, l, a numerical aperture (NA), magnification of the objective, radius of the confocal pinhole, refractive index of the object, etc. Once this “optical slicing” has been achieved, the objective (or the sample stage) is moved along the optical axis of the microscope to obtain a series of 2D optically sliced images, which is later used to reconstruct a 3D image (see Sect. 3.1 for details). To our best knowledge, Verhoogt et al. [7] first reported an application of LSCM to a polymer mixture. Although their work was instrument oriented and thus did not provide much insight into the phase-separated structure of the binary mixture itself, the potential of the instrument was clearly demonstrated. Image generation in LSCM of a polymer blend system was discussed by Ribbe et al. [8]. White and Wiltzius [9] discussed a mechanism of the phase separation in an off-critical polymer mixture through the time evolution of the size distribution of spherical domains. LSCM was applied to investigate the phase-separated structure of polymer mixtures at the critical composition, demonstrating that the structure is truly interconnected and periodically arranged, forming a 3D “maze” [10–12]. These studies are considered to take full advantage of 3D reconstruction intrinsic to LSCM. Morphology under a shear flow [13] and that of a ternary polymer mixture [14] were also studied by LSCM. We note that some other studies rather use the excellent depth resolution of the confocal microscope; surface and bulk structures of the solvent-cast films of a polymer mixture were investigated as a function of distance from the air–polymer surface [15, 16]. LSCM was also applied to investigate and demonstrate the penetration process of a spherulite into another spherulite of a different component in crystalline/crystalline polymer blends [17]. Besides those studies, LSCM was used for structural investigation of gel [18, 19], membrane systems [20, 21].

Emerging Technologies for the 3D Analysis of Polymer Structures

123

2.2 Transmission Electron Microtomography (TEMT) As already mentioned, TEMT is a method to image structures in 3D at nanometer-scale resolution [22]. Unlike confocal microscopy, TEMT uses a series of 2D projections taken by transmission electron microscopy (TEM) that are subsequently used to compute a 3D image of the object on the basis of computerized tomography (CT). TEMT offers a new approach to obtain 3D information of the order of the nanometer scale, and hence was rapidly developed during the past few years first in the biological community. Although the high potential of TEMT as a unique and powerful tool to study various types of structures in material science was recognized [23], it is only recently that the technique became available to the material community [24, 25]. So far, only a few studies [26–30] have used TEMT to investigate the complex 3D structures of polymeric materials, most of which dealt with the microphase-separated structures of block copolymers [see Sect. 5 for an example]. In what follows we will describe the principles of CT and subsequently discuss several experimental limitations in the TEMT measurements. The CT allows the complete 3D internal structure of an object to be reconstructed from a set of 2D projections at different angular settings, without imposing any a priori assumptions or requirements regarding the symmetry of the object. The reconstruction from projections is aided by an understanding of the relationship between an object and its projections in Fourier space: “the central slice theorem” [31] states that the Fourier transform of an objects projection is a central plane in the Fourier transform of the object as shown in Fig. 3. A projection of a 2D object, represented by the function f(x,y), is produced by parallel illumination from the electron source passing through the object, which is tilted at an angle j about an axis orthogonal to the beam path. p(r,j) denotes the projection in real space. The Fourier transform of p(r,j) is Z þ1 Fðq; jÞ ¼ pðr; jÞeiqr dr: ð1Þ 1

Here q is the wave number. The Fourier coefficients, F(q,f), are arranged along the line in Fourier space with the same tilting angle f. Gathering 2D projections over as wide a tilting range as possible gives a 3D Fourier transform of the object. Note that the ideal 180 range of tilt is required to give a complete sampling of Fourier space. Taking the inverse Fourier transform of the entire array of coefficients results in the reconstructed volume in real space. In the above 2D object case (in Fig. 3):

124

H. Jinnai et al.

Fig. 3 The discrete form of the central slice theorem in two dimensions. A projection p(r,j) in real space (x,y) at angle j is a slice F(q,j) at the same angle in Fourier space (qx,qy)

f ðx; yÞ ¼

2p Z þ1

Z 0

Fðq; jÞeiqðxcosjþysinjÞ qdqdj:

ð2Þ

0

Unfortunately the projection data are always sampled at discrete angles leaving regular gaps in Fourier space. The inverse Fourier transform intrinsically requires a continuous function, and therefore azimuthal interpolation is required to fill the gaps in Fourier space. The quality of the reconstruction is significantly affected by the type of interpolation implemented [32]. An alternative and more commonly used algorithm is the radius-weighted back projection technique [33]. In the case of TEMT, the projections at different angles are collected by tilting the specimen with respect to the electron beam in the TEM column. The tilt range achievable in a TEM is restricted by the relative geometries of specimen holder and objective lens since they will contact physically at high tilt angle, e.g., 70. The missing information due to this limitation becomes a wedge-shaped region of Fourier space, giving rise to a loss of resolution in the reconstructed image especially in the direction parallel to the electron beam. The restoration of the missing structural information has been studied intensively [34]. In addition, the resolution of the reconstructed image is strongly affected by the numbers of projections. The resolution is expressed as [35], r ¼ pDCT =NCT ;

ð3Þ

where r is the size of the smallest feature visualized in the reconstruction. DCT and NCT are the diameter (size) of the object or feature being reconstructed and the number of projections, respectively. Since the Fourier coefficients are radially arranged, more information will be lost as q increases, which limits the resolution of the reconstructed images. Equation 3 tells us that the resolution will be compensated by increasing the number of projec-

Emerging Technologies for the 3D Analysis of Polymer Structures

125

tions gathered; since NCT is increased, the density of the Fourier coefficients at a given q will be more dense. In reality, however, the angular increment in TEMT experiments is also limited to, at smallest, 1 (typically 2) due to the severe electron beam damage to the polymer specimens. During tilting the specimen, misalignments in the digitized images are also inevitable due to the imperfect eucentricity of the specimen stage. As a crucial prelude to calculating a 3D reconstruction, alignment of the digitized images is necessary. This is achieved either by least squares tracking of fiducial markers [22], such as small gold particles, or by sequential cross-correlation. Often a combination of both processes is used [36].

3 Digital Image Analysis of 3D Structures In the preceding section, two types of 3D microscopy were introduced. In some cases, it is sufficient to have 3D images of the structures in order to intuitively grasp their unique features. Actually, many researchers, in material science as well as in the medical and biological fields, seem to be content with 3D “pretty” pictures or the cross-sectional views of their 3D objects. This is merely “observations”, not “structural analysis”. Yet 3D microscopy gives much more structural information than either the conventional 2D microscopes or the scattering methods, most of which have never been acquired before. It is expected that the new structural information will clear up the root of unsolved physical problems. In the present section, we will introduce some quantitative analytical methods to extract such structural parameters from the 3D digital data. 3.1 3D Reconstruction In most cases, a 3D image is constructed from a stack of two-dimensional (2D) slices, i.e., a 3D array of image intensities. In the case of fluorescent LSCM, for example, the image intensities correspond to the concentration of fluorescent molecules that are chemically attached to one of the constituents. For quantitative image analysis, it is first necessary to isolate the portions of interest by defining surfaces that separate such particular parts from the other parts of the structures. The surfaces are called “interface”. One can assign the interface by specifying a threshold value for the image intensities. The marching cubes algorithm (MCA) [37] is used to find the interface from the 3D image. In this algorithm, a cube is created from the centers of eight adjacent pixels; four pixels from each of two adjacent slices. The image intensity at the pixels is assigned to the corresponding vertices of the cube. The interface is considered to intersect an edge of this cube if the in-

126

H. Jinnai et al.

tensity of one vertex of this edge is larger than the threshold value, and that of another vertex of the same edge is smaller than the threshold value. An intersecting point between the interface and the edge of the cube is determined by a linear interpolation according to the image intensity assigned to the two vertices on the edge. By properly connecting the intersections determined for the cube, the local interface is constructed and represented by a set of triangles. Note that the MCA defines the 14 types of intersection for the interface constructed in the cube by taking rotational and mirror symmetry into consideration (see Fig. 3 in ref. [37]). This gives a polygonal representation of the interface, which eventually reduces to triangles, from the 3D array of data by the MCA. A normal vector of each triangle, ntri, can be estimated by ntri ¼

ðp2 p1 Þ ðp3 p2 Þ ; jðp2 p1 Þ ðp3 p2 Þj

ð4Þ

where p1, p2, and p3 are the positional vectors of the vertices of the triangle. The normal vectors thus obtained from the MCA were used to evaluate normal vectors at vertices of the polygon, n. We note that the normal vectors obtained by the MCA, i.e., ntri, were those for the triangles comprising the polygon, not for the vertices. n was estimated by averaging the normal vectors of the neighboring triangles that shared the vertex of interest with those areas as a weighting: P i Si ntri : n ¼ i ð5Þ P Si ni tri i

Here nitri and Si denote, respectively, the normal vector and the area of the i-th neighboring triangle. Equation 5 will be further used to generate a parallel surface to measure surface curvatures (see Sect. 3.2.2 for details). 3.2 Curvature Distribution Measurements In some systems, the local shape of surfaces is significant in understanding the formation and stability of the morphologies and thus it can be a key structural measure to clarify the underlying physics. Surface curvatures are fundamental parameters characterizing the shape of surfaces in the differential geometry. From the volume data taken by the 3D microscopy, it is possible to determine the surface curvatures for the first time.

Emerging Technologies for the 3D Analysis of Polymer Structures

127

3.2.1 Surface Curvatures The curvatures at an arbitrary point on the surface can be expressed by two principal curvatures or the mean and Gaussian curvatures [38]. A 2D curvature is defined for a planar-curved path passing through a point of interest (POI) on the surface. The path is expressed by the intersection between the surface and the plane contains the surface normal vector at the point (see Fig. 4). Paths with different tangential directions on the surface have, in general, different values for the curvatures. Maximum and minimum values among those curvatures at the point of interest are called the principal curvatures, i.e., k1 and k2, as schematically shown in Figs. 4 and 7. Note that each curvature has a sign: it is positive if the path is convex from one side, negative otherwise, and zero if the path is straight. The mean curvature, H, and the Gaussian curvature, K, are defined as H¼

k1 þ k2 ; K ¼ k1 k2 : 2

ð6Þ

They are uniquely determined at the point p. The sign of K classifies the shape of the surface: it is elliptic if K>0, parabolic if K=0, and hyperbolic if K

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close